# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2020

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1
_database_code_depnum_ccdc_archive 'CCDC 1961645'
loop_
_audit_author_name
_audit_author_address
'hui xu'
;Jilin University
China
;
_audit_update_record             
;
2019-10-28 deposited with the CCDC.	2019-12-17 downloaded from the CCDC.
;
_audit_creation_date             2019-10-21
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2018/3
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         
'Ge2 H4 Mo20 Ni4 O74, C12 H36 N24 Ni3 O6, 10(H2 O)'
_chemical_formula_sum            'C12 H60 Ge2 Mo20 N24 Ni7 O90'
_chemical_formula_weight         4455.69
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   13.9330(19)
_cell_length_b                   14.2147(19)
_cell_length_c                   14.591(2)
_cell_angle_alpha                110.716(2)
_cell_angle_beta                 98.574(2)
_cell_angle_gamma                112.773(2)
_cell_volume                     2351.2(6)
_cell_formula_units_Z            1
_cell_measurement_reflns_used    5368
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.259
_cell_measurement_theta_min      2.510
_shelx_estimated_absorpt_T_max   0.521
_shelx_estimated_absorpt_T_min   0.353
_exptl_absorpt_coefficient_mu    4.692
_exptl_absorpt_correction_T_max  0.472
_exptl_absorpt_correction_T_min  0.319
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            'pale green'
_exptl_crystal_colour_primary    'pale green'
_exptl_crystal_density_diffrn    3.147
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             2120
_exptl_crystal_size_max          0.28
_exptl_crystal_size_mid          0.21
_exptl_crystal_size_min          0.16
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0243
_diffrn_reflns_av_unetI/netI     0.0489
_diffrn_reflns_Laue_measured_fraction_full 0.992
_diffrn_reflns_Laue_measured_fraction_max 0.987
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -18
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            17517
_diffrn_reflns_point_group_measured_fraction_full 0.992
_diffrn_reflns_point_group_measured_fraction_max 0.987
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         28.322
_diffrn_reflns_theta_min         1.680
_diffrn_ambient_temperature      296.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.992
_diffrn_measured_fraction_theta_max 0.987
_diffrn_measurement_device_type  'CCD Area Detector'
_diffrn_measurement_method       ?
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                9154
_reflns_number_total             11710
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT v8.34A (Bruker, 2013)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT v8.34A (Bruker, 2013)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    ?
_refine_diff_density_max         1.355
_refine_diff_density_min         -1.125
_refine_diff_density_rms         0.191
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.039
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     720
_refine_ls_number_reflns         11563
_refine_ls_number_restraints     36
_refine_ls_R_factor_all          0.0483
_refine_ls_R_factor_gt           0.0351
_refine_ls_restrained_S_all      1.043
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0380P)²+1.8274P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0824
_refine_ls_wR_factor_ref         0.0893
_refine_special_details          ?
_olex2_refinement_description    
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, {H1WA,H1WB} of O1W, {H5WA,H5WB} of O5W, All N(H,H) groups
 At 1.5 times of:
  {H2WA,H2WB} of O2W, {H3WA,H3WB} of O3W, {H10A,H10B} of O10W, {H6WA,H6WB} of
  O6W, {H8WA,H8WB} of O8W, {H9WA,H9WB} of O9W, {H4WA,H4WB} of O4W, {H7WA,H7WB}
  of O7W, {H7WC,H7WD} of O7WA
2. Uiso/Uaniso restraints and constraints
Uanis(O7W) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
Uanis(O7WA) \\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.01
Uanis(O9W) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
Uanis(O8W) \\sim Ueq, Uanis(O9W) \\sim Ueq, Uanis(O6W) \\sim Ueq, Uanis(O4W)
\\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
3. Others
 Sof(O7WA)=Sof(H7WC)=Sof(H7WD)=1-FVAR(1)
 Sof(O7W)=Sof(H7WA)=Sof(H7WB)=FVAR(1)
 Fixed Sof: O8W(0.5) H8WA(0.5) H8WB(0.5) O9W(0.5) H9WA(0.5) H9WB(0.5)
4.a Riding coordinates:
 O10W(H10A,H10B), O1W(H1WA,H1WB), O2W(H2WA,H2WB), O4W(H4WA,H4WB), O5W(H5WA,
 H5WB), O6W(H6WA,H6WB), O7W(H7WA,H7WB), O7WA(H7WC,H7WD), O8W(H8WA,H8WB),
 O9W(H9WA,H9WB)
4.b Rotating group:
 O3W(H3WA,H3WB)
4.c Aromatic/amide H refined with riding coordinates:
 C1(H1), C2(H2), C3(H3), C4(H4), C5(H5), C6(H6)
4.d X=CH2 refined with riding coordinates:
 N2(H2A,H2B), N3(H3A,H3B), N4(H4A,H4B)
;
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo -0.04186(4) 0.55411(4) 0.19648(3) 0.01507(10) Uani 1 1 d . . . . .
Mo2 Mo 0.00199(3) 0.70901(4) 0.46621(3) 0.01332(9) Uani 1 1 d . . . . .
Mo3 Mo 0.12656(3) 0.91945(4) 0.17514(3) 0.01463(9) Uani 1 1 d . . . . .
Mo4 Mo 0.27636(3) 1.29527(4) 0.60745(3) 0.01369(9) Uani 1 1 d . . . . .
Mo5 Mo -0.09878(4) 0.66706(4) 0.01159(3) 0.01491(9) Uani 1 1 d . . . . .
Mo6 Mo 0.11241(4) 1.08521(4) 0.88796(3) 0.01492(10) Uani 1 1 d . . . . .
Mo7 Mo 0.32308(3) 1.19939(4) 0.77854(3) 0.01473(9) Uani 1 1 d . . . . .
Mo8 Mo -0.31596(3) 0.55084(4) 0.12434(3) 0.01513(10) Uani 1 1 d . . . . .
Mo9 Mo 0.18373(3) 0.80868(4) 0.35685(3) 0.01384(9) Uani 1 1 d . . . . .
Mo10 Mo -0.23078(4) 0.48450(4) 0.30340(4) 0.01793(10) Uani 1 1 d . . . . .
Ge1 Ge 0.06534(4) 1.18678(4) 0.70665(4) 0.01008(10) Uani 1 1 d . . . . .
Ni1 Ni 0.11378(5) 1.00187(5) 0.53074(5) 0.01300(13) Uani 1 1 d . . . . .
Ni2 Ni -0.06346(5) 0.90814(5) 0.62560(5) 0.01461(14) Uani 1 1 d . . . . .
O1 O -0.2509(4) 0.4646(3) 0.4112(3) 0.0313(10) Uani 1 1 d . . . . .
O2 O -0.4097(3) 0.4124(3) 0.0478(3) 0.0251(9) Uani 1 1 d . . . . .
O3 O -0.1368(3) 0.5672(3) -0.1104(3) 0.0239(9) Uani 1 1 d . . . . .
O4 O 0.1600(3) 1.0362(3) 0.9650(3) 0.0243(9) Uani 1 1 d . . . . .
O5 O 0.3134(3) 0.8229(3) 0.3845(3) 0.0247(9) Uani 1 1 d . . . . .
O6 O 0.3430(3) 1.3503(3) 0.5360(3) 0.0264(9) Uani 1 1 d . . . . .
O7 O -0.0707(3) 0.4157(3) 0.1369(3) 0.0234(8) Uani 1 1 d . . . . .
O8 O -0.0501(3) 0.5961(3) 0.0935(3) 0.0190(8) Uani 1 1 d . . . . .
O9 O 0.2419(3) 0.9728(3) 0.1451(3) 0.0234(8) Uani 1 1 d . . . . .
O10 O 0.1659(3) 0.8303(3) 0.2397(3) 0.0195(8) Uani 1 1 d . . . . .
O11 O -0.1889(3) 0.5394(3) 0.1881(3) 0.0173(8) Uani 1 1 d . . . . .
O12 O 0.1063(3) 0.6311(3) 0.2613(3) 0.0182(8) Uani 1 1 d . . . . .
O13 O 0.3743(3) 1.2700(3) 0.6786(3) 0.0205(8) Uani 1 1 d . . . . .
O14 O 0.1508(3) 1.0270(3) 0.2950(3) 0.0194(8) Uani 1 1 d . . . . .
O15 O -0.0020(3) 1.2601(3) 0.6781(3) 0.0129(7) Uani 1 1 d . . . . .
O10W O -0.1407(3) 0.7617(3) 0.6401(3) 0.0252(9) Uani 1 1 d . . . . .
H10A H -0.208035 0.718720 0.596573 0.038 Uiso 1 1 d R . . . .
H10B H -0.105385 0.721770 0.623603 0.038 Uiso 1 1 d R . . . .
O17 O -0.2867(3) 0.3475(3) 0.2091(3) 0.0296(10) Uani 1 1 d . . . . .
O18 O 0.1386(3) 0.7363(3) 0.4557(3) 0.0184(8) Uani 1 1 d . . . . .
O19 O 0.2523(3) 1.1735(3) 0.8719(3) 0.0172(8) Uani 1 1 d . . . . .
O20 O -0.0040(3) 0.6506(3) 0.5495(3) 0.0231(8) Uani 1 1 d . . . . .
O21 O 0.0581(3) 0.9733(3) 0.7617(3) 0.0200(8) Uani 1 1 d . . . . .
O22 O -0.3366(3) 0.5372(3) 0.2644(3) 0.0201(8) Uani 1 1 d . . . . .
O23 O 0.4387(3) 1.1910(3) 0.8177(3) 0.0259(9) Uani 1 1 d . . . . .
O24 O 0.2076(3) 1.2626(3) 0.7338(3) 0.0130(7) Uani 1 1 d . . . . .
O25 O 0.1974(3) 0.9361(3) 0.4480(3) 0.0169(7) Uani 1 1 d . . . . .
O26 O -0.0699(3) 0.5414(3) 0.3330(3) 0.0167(7) Uani 1 1 d . . . . .
O27 O 0.0447(3) 0.7619(3) 0.0404(3) 0.0180(8) Uani 1 1 d . . . . .
O28 O 0.0324(3) 0.9521(3) 0.0967(3) 0.0174(8) Uani 1 1 d . . . . .
O29 O -0.3974(3) 0.6247(3) 0.1295(3) 0.0198(8) Uani 1 1 d . . . . .
O30 O -0.1549(3) 0.7585(3) -0.0098(3) 0.0166(7) Uani 1 1 d . . . . .
O31 O 0.0300(3) 0.8533(3) 0.5427(3) 0.0173(7) Uani 1 1 d . . . . .
O32 O -0.2411(3) 0.5927(3) 0.0433(3) 0.0184(8) Uani 1 1 d . . . . .
O33 O -0.1536(3) 0.6672(3) 0.4092(3) 0.0156(7) Uani 1 1 d . . . . .
O34 O 0.1803(3) 1.1497(3) 0.5149(3) 0.0165(7) Uani 1 1 d . . . . .
O35 O 0.0113(3) 1.0505(3) 0.6027(3) 0.0120(7) Uani 1 1 d . . . . .
O36 O 0.2377(3) 1.0683(3) 0.6660(3) 0.0188(8) Uani 1 1 d . . . . .
O37 O 0.0465(3) 1.1795(3) 0.8207(3) 0.0126(7) Uani 1 1 d . . . . .
Ni3 Ni 0.500000 1.000000 1.000000 0.01447(19) Uani 1 2 d S T P . .
Ni4 Ni 0.44405(6) 0.89363(6) 0.71470(5) 0.02050(15) Uani 1 1 d . . . . .
O1W O 0.3410(4) 0.7379(4) 0.5865(3) 0.0466(13) Uani 1 1 d . . . . .
H1WA H 0.283469 0.737800 0.557141 0.056 Uiso 1 1 d R . . . .
H1WB H 0.321799 0.683890 0.603871 0.056 Uiso 1 1 d R . . . .
O2W O 0.3821(4) 0.9575(4) 0.6249(3) 0.0367(11) Uani 1 1 d . . . . .
H2WA H 0.363268 0.928277 0.556700 0.055 Uiso 1 1 d R . . . .
H2WB H 0.341258 0.988477 0.647950 0.055 Uiso 1 1 d R . . . .
O3W O 0.5634(4) 0.8984(4) 0.6410(3) 0.0410(12) Uani 1 1 d . . . . .
H3WA H 0.628894 0.958620 0.681002 0.061 Uiso 1 1 d GR . . . .
H3WB H 0.548462 0.910341 0.586151 0.061 Uiso 1 1 d GR . . . .
N1 N 0.5685(4) 0.7322(4) 0.8538(4) 0.0282(11) Uani 1 1 d . . . . .
N2 N 0.0565(4) 0.7648(4) 0.8063(4) 0.0366(13) Uani 1 1 d . . . . .
H2A H 0.008168 0.722026 0.745118 0.044 Uiso 1 1 calc R . . . .
H2B H 0.036040 0.773301 0.860111 0.044 Uiso 1 1 calc R . . . .
N3 N 0.7611(4) 1.3400(4) 0.9104(4) 0.0376(14) Uani 1 1 d . . . . .
H3A H 0.776448 1.349546 0.858316 0.045 Uiso 1 1 calc R . . . .
H3B H 0.795686 1.395613 0.972085 0.045 Uiso 1 1 calc R . . . .
N4 N 0.6022(5) 0.6486(5) 0.8512(5) 0.0460(16) Uani 1 1 d . . . . .
H4A H 0.623276 0.644303 0.907349 0.055 Uiso 1 1 calc R . . . .
H4B H 0.601282 0.602498 0.793420 0.055 Uiso 1 1 calc R . . . .
N5 N 0.1685(3) 0.8207(4) 0.8182(4) 0.0234(10) Uani 1 1 d . . . . .
N6 N 0.5082(4) 0.8288(4) 0.8000(4) 0.0230(10) Uani 1 1 d . . . . .
N7 N 0.5724(3) 1.1011(4) 0.9285(3) 0.0165(9) Uani 1 1 d . . . . .
N8 N 0.5287(3) 0.8700(4) 0.9059(3) 0.0186(9) Uani 1 1 d . . . . .
N9 N 0.5528(3) 1.0567(4) 0.8235(3) 0.0153(9) Uani 1 1 d . . . . .
N10 N 0.6793(3) 1.2332(4) 0.8946(3) 0.0182(9) Uani 1 1 d . . . . .
N11 N 0.3470(3) 0.9259(4) 0.8899(3) 0.0179(9) Uani 1 1 d . . . . .
N12 N 0.3220(4) 0.8794(4) 0.7838(3) 0.0223(10) Uani 1 1 d . . . . .
C1 C 0.2149(5) 0.8174(5) 0.7441(5) 0.0286(13) Uani 1 1 d . . . . .
H1 H 0.175896 0.776234 0.673278 0.034 Uiso 1 1 calc R . . . .
C2 C 0.5649(5) 0.8099(5) 0.9363(5) 0.0251(12) Uani 1 1 d . . . . .
H2 H 0.584722 0.819635 1.004003 0.030 Uiso 1 1 calc R . . . .
C3 C 0.5345(5) 0.7468(5) 0.7712(5) 0.0271(13) Uani 1 1 d . . . . .
H3 H 0.530287 0.704906 0.703927 0.033 Uiso 1 1 calc R . . . .
C4 C 0.2539(4) 0.8908(5) 0.9092(4) 0.0224(12) Uani 1 1 d . . . . .
H4 H 0.247217 0.910778 0.975033 0.027 Uiso 1 1 calc R . . . .
C5 C 0.6171(4) 1.1373(4) 0.8050(4) 0.0196(11) Uani 1 1 d . . . . .
H5 H 0.619786 1.129823 0.739589 0.023 Uiso 1 1 calc R . . . .
C6 C 0.6478(4) 1.2083(4) 0.9699(4) 0.0179(11) Uani 1 1 d . . . . .
H6 H 0.675376 1.259354 1.040115 0.021 Uiso 1 1 calc R . . . .
O4W O -0.1469(6) 0.8107(4) 0.8280(4) 0.075(2) Uani 1 1 d . U . . .
H4WA H -0.158748 0.771336 0.763994 0.112 Uiso 1 1 d R . . . .
H4WB H -0.162438 0.769216 0.859234 0.112 Uiso 1 1 d R . . . .
O5W O 0.1336(5) 0.4831(6) 0.3611(5) 0.083(2) Uani 1 1 d . . . . .
H5WA H 0.111823 0.519847 0.336081 0.099 Uiso 1 1 d R . . . .
H5WB H 0.085113 0.449127 0.383591 0.099 Uiso 1 1 d R . . . .
O6W O -0.6129(5) 0.5832(6) 0.1884(7) 0.114(3) Uani 1 1 d . U . . .
H6WA H -0.682685 0.551559 0.176886 0.171 Uiso 1 1 d R . . . .
H6WB H -0.575035 0.580719 0.145766 0.171 Uiso 1 1 d R . . . .
O7W O 0.5349(7) 0.8637(10) 0.4444(6) 0.058(4) Uani 0.650(16) 1 d . U . A 1
H7WA H 0.555093 0.825163 0.402831 0.087 Uiso 0.650(16) 1 d R . . A 1
H7WB H 0.467413 0.841493 0.419541 0.087 Uiso 0.650(16) 1 d R . . A 1
O7WA O 0.4799(14) 0.7639(18) 0.4339(13) 0.063(7) Uani 0.350(16) 1 d . U . A 2
H7WC H 0.511766 0.756572 0.388317 0.095 Uiso 0.350(16) 1 d R . . A 2
H7WD H 0.428246 0.779362 0.419517 0.095 Uiso 0.350(16) 1 d R . . A 2
O8W O -0.3255(9) 0.5237(11) 0.6751(9) 0.077(4) Uani 0.5 1 d . U . . .
H8WA H -0.276610 0.505934 0.676215 0.116 Uiso 0.5 1 d R . . . .
H8WB H -0.351420 0.509014 0.612275 0.116 Uiso 0.5 1 d R . . . .
O9W O -0.4715(12) 0.4187(13) 0.4715(11) 0.134(7) Uani 0.5 1 d . U . B -1
H9WA H -0.465852 0.483277 0.480510 0.201 Uiso 0.5 1 d R . . B -1
H9WB H -0.517912 0.403087 0.505390 0.201 Uiso 0.5 1 d R . . B -1


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O7 1.692(4) . ?
Mo1 O8 1.807(4) . ?
Mo1 O11 1.957(3) . ?
Mo1 O12 1.813(3) . ?
Mo1 O15 2.387(3) 2_576 ?
Mo1 O26 2.141(4) . ?
Mo2 O15 2.298(3) 2_576 ?
Mo2 O18 1.832(4) . ?
Mo2 O20 1.693(4) . ?
Mo2 O26 2.180(3) . ?
Mo2 O31 1.799(3) . ?
Mo2 O33 1.964(3) . ?
Mo3 O9 1.689(4) . ?
Mo3 O10 2.006(4) . ?
Mo3 O14 1.745(4) . ?
Mo3 O27 2.103(3) . ?
Mo3 O28 1.909(3) . ?
Mo3 O37 2.297(3) 2_576 ?
Mo4 O6 1.692(4) . ?
Mo4 O13 1.815(4) . ?
Mo4 O22 2.170(4) 2_576 ?
Mo4 O24 2.306(3) . ?
Mo4 O33 1.986(3) 2_576 ?
Mo4 O34 1.799(3) . ?
Mo5 O3 1.678(4) . ?
Mo5 O8 2.011(4) . ?
Mo5 O27 1.804(4) . ?
Mo5 O30 1.844(3) . ?
Mo5 O32 2.064(4) . ?
Mo5 O37 2.396(3) 2_576 ?
Mo6 O4 1.697(4) . ?
Mo6 O19 1.970(4) . ?
Mo6 O21 1.754(4) . ?
Mo6 O28 1.948(3) 2_576 ?
Mo6 O30 2.079(3) 2_576 ?
Mo6 O37 2.285(3) . ?
Mo7 O13 2.105(4) . ?
Mo7 O19 1.854(4) . ?
Mo7 O23 1.690(4) . ?
Mo7 O24 2.245(3) . ?
Mo7 O29 2.082(3) 2_576 ?
Mo7 O36 1.767(4) . ?
Mo8 O2 1.687(4) . ?
Mo8 O11 1.966(3) . ?
Mo8 O22 2.170(4) . ?
Mo8 O24 2.384(3) 2_576 ?
Mo8 O29 1.812(4) . ?
Mo8 O32 1.796(4) . ?
Mo9 O5 1.706(4) . ?
Mo9 O10 1.839(4) . ?
Mo9 O12 2.106(3) . ?
Mo9 O15 2.230(3) 2_576 ?
Mo9 O18 2.087(4) . ?
Mo9 O25 1.743(3) . ?
Mo10 O1 1.737(4) . ?
Mo10 O11 2.156(4) . ?
Mo10 O17 1.704(4) . ?
Mo10 O22 1.991(4) . ?
Mo10 O26 1.982(4) . ?
Mo10 O33 2.189(3) . ?
Ge1 O15 1.757(3) . ?
Ge1 O24 1.749(3) . ?
Ge1 O35 1.753(3) . ?
Ge1 O37 1.755(3) . ?
Ni1 O25 2.038(3) . ?
Ni1 O31 2.065(4) . ?
Ni1 O34 2.056(4) . ?
Ni1 O35 2.077(3) . ?
Ni1 O35 2.083(3) 2_576 ?
Ni1 O36 2.042(3) . ?
Ni2 O14 2.050(4) 2_576 ?
Ni2 O10W 2.045(4) . ?
Ni2 O21 2.037(4) . ?
Ni2 O31 2.086(4) . ?
Ni2 O34 2.075(3) 2_576 ?
Ni2 O35 2.060(3) . ?
O10W H10A 0.8720 . ?
O10W H10B 0.8822 . ?
Ni3 N7 2.103(4) . ?
Ni3 N7 2.103(4) 2_677 ?
Ni3 N8 2.098(4) 2_677 ?
Ni3 N8 2.098(4) . ?
Ni3 N11 2.068(4) 2_677 ?
Ni3 N11 2.068(4) . ?
Ni4 O1W 2.067(4) . ?
Ni4 O2W 2.097(4) . ?
Ni4 O3W 2.103(4) . ?
Ni4 N6 2.077(5) . ?
Ni4 N9 2.037(4) . ?
Ni4 N12 2.084(5) . ?
O1W H1WA 0.8498 . ?
O1W H1WB 0.8505 . ?
O2W H2WA 0.8809 . ?
O2W H2WB 0.8824 . ?
O3W H3WA 0.8883 . ?
O3W H3WB 0.8864 . ?
N1 N4 1.427(7) . ?
N1 C2 1.340(7) . ?
N1 C3 1.342(8) . ?
N2 H2A 0.8600 . ?
N2 H2B 0.8600 . ?
N2 N5 1.400(6) . ?
N3 H3A 0.8600 . ?
N3 H3B 0.8600 . ?
N3 N10 1.412(6) . ?
N4 H4A 0.8600 . ?
N4 H4B 0.8600 . ?
N5 C1 1.336(8) . ?
N5 C4 1.359(7) . ?
N6 N8 1.382(6) . ?
N6 C3 1.304(7) . ?
N7 N9 1.370(6) . ?
N7 C6 1.308(6) . ?
N8 C2 1.308(7) . ?
N9 C5 1.299(7) . ?
N10 C5 1.343(6) . ?
N10 C6 1.351(7) . ?
N11 N12 1.375(6) . ?
N11 C4 1.311(7) . ?
N12 C1 1.304(7) . ?
C1 H1 0.9300 . ?
C2 H2 0.9300 . ?
C3 H3 0.9300 . ?
C4 H4 0.9300 . ?
C5 H5 0.9300 . ?
C6 H6 0.9300 . ?
O4W H4WA 0.8514 . ?
O4W H4WB 0.8506 . ?
O5W H5WA 0.8497 . ?
O5W H5WB 0.8499 . ?
O6W H6WA 0.8579 . ?
O6W H6WB 0.8729 . ?
O7W H7WA 0.8262 . ?
O7W H7WB 0.8383 . ?
O7WA H7WC 0.8518 . ?
O7WA H7WD 0.8483 . ?
O8W H8WA 0.8129 . ?
O8W H8WB 0.8501 . ?
O9W H9WA 0.8500 . ?
O9W H9WB 0.8798 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O7 Mo1 O8 104.85(18) . . ?
O7 Mo1 O11 101.72(16) . . ?
O7 Mo1 O12 104.04(17) . . ?
O7 Mo1 O15 164.05(16) . 2_576 ?
O7 Mo1 O26 92.29(16) . . ?
O8 Mo1 O11 86.58(16) . . ?
O8 Mo1 O12 100.06(16) . . ?
O8 Mo1 O15 91.10(14) . 2_576 ?
O8 Mo1 O26 156.39(15) . . ?
O11 Mo1 O15 78.45(13) . 2_576 ?
O11 Mo1 O26 73.93(14) . . ?
O12 Mo1 O11 150.66(15) . . ?
O12 Mo1 O15 72.92(13) . 2_576 ?
O12 Mo1 O26 91.16(15) . . ?
O26 Mo1 O15 72.31(12) . 2_576 ?
O18 Mo2 O15 75.15(14) . 2_576 ?
O18 Mo2 O26 89.42(14) . . ?
O18 Mo2 O33 152.70(16) . . ?
O20 Mo2 O15 164.27(15) . 2_576 ?
O20 Mo2 O18 101.17(17) . . ?
O20 Mo2 O26 91.39(16) . . ?
O20 Mo2 O31 105.19(17) . . ?
O20 Mo2 O33 101.44(16) . . ?
O26 Mo2 O15 73.43(12) . 2_576 ?
O31 Mo2 O15 90.53(14) . 2_576 ?
O31 Mo2 O18 99.67(16) . . ?
O31 Mo2 O26 159.00(15) . . ?
O31 Mo2 O33 88.95(15) . . ?
O33 Mo2 O15 78.94(13) . 2_576 ?
O33 Mo2 O26 74.95(13) . . ?
O9 Mo3 O10 98.57(17) . . ?
O9 Mo3 O14 104.66(18) . . ?
O9 Mo3 O27 95.85(16) . . ?
O9 Mo3 O28 100.55(17) . . ?
O9 Mo3 O37 167.87(15) . 2_576 ?
O10 Mo3 O27 83.74(14) . . ?
O10 Mo3 O37 84.21(13) . 2_576 ?
O14 Mo3 O10 92.93(16) . . ?
O14 Mo3 O27 159.49(15) . . ?
O14 Mo3 O28 94.97(16) . . ?
O14 Mo3 O37 86.91(14) . 2_576 ?
O27 Mo3 O37 72.63(13) . 2_576 ?
O28 Mo3 O10 156.71(15) . . ?
O28 Mo3 O27 81.21(14) . . ?
O28 Mo3 O37 74.40(13) . 2_576 ?
O6 Mo4 O13 103.83(18) . . ?
O6 Mo4 O22 92.88(16) . 2_576 ?
O6 Mo4 O24 166.98(16) . . ?
O6 Mo4 O33 99.56(17) . 2_576 ?
O6 Mo4 O34 103.59(17) . . ?
O13 Mo4 O22 90.86(15) . 2_576 ?
O13 Mo4 O24 75.25(14) . . ?
O13 Mo4 O33 153.02(15) . 2_576 ?
O22 Mo4 O24 74.21(13) 2_576 . ?
O33 Mo4 O22 74.60(14) 2_576 2_576 ?
O33 Mo4 O24 78.92(13) 2_576 . ?
O34 Mo4 O13 98.93(16) . . ?
O34 Mo4 O22 158.12(15) . 2_576 ?
O34 Mo4 O24 89.33(14) . . ?
O34 Mo4 O33 88.35(15) . 2_576 ?
O3 Mo5 O8 101.08(17) . . ?
O3 Mo5 O27 103.81(17) . . ?
O3 Mo5 O30 101.35(17) . . ?
O3 Mo5 O32 98.34(16) . . ?
O3 Mo5 O37 174.88(16) . 2_576 ?
O8 Mo5 O32 80.34(14) . . ?
O8 Mo5 O37 83.98(13) . 2_576 ?
O27 Mo5 O8 88.33(15) . . ?
O27 Mo5 O30 97.61(16) . . ?
O27 Mo5 O32 156.71(15) . . ?
O27 Mo5 O37 75.39(13) . 2_576 ?
O30 Mo5 O8 154.65(15) . . ?
O30 Mo5 O32 84.87(15) . . ?
O30 Mo5 O37 73.85(13) . 2_576 ?
O32 Mo5 O37 83.18(12) . 2_576 ?
O4 Mo6 O19 98.65(17) . . ?
O4 Mo6 O21 105.05(18) . . ?
O4 Mo6 O28 99.45(17) . 2_576 ?
O4 Mo6 O30 94.66(16) . 2_576 ?
O4 Mo6 O37 166.08(15) . . ?
O19 Mo6 O30 83.55(14) . 2_576 ?
O19 Mo6 O37 85.44(13) . . ?
O21 Mo6 O19 94.61(16) . . ?
O21 Mo6 O28 93.18(16) . 2_576 ?
O21 Mo6 O30 160.25(15) . 2_576 ?
O21 Mo6 O37 87.78(15) . . ?
O28 Mo6 O19 157.69(15) 2_576 . ?
O28 Mo6 O30 82.09(14) 2_576 2_576 ?
O28 Mo6 O37 74.00(13) 2_576 . ?
O30 Mo6 O37 72.48(13) 2_576 . ?
O13 Mo7 O24 71.56(13) . . ?
O19 Mo7 O13 157.53(15) . . ?
O19 Mo7 O24 87.34(14) . . ?
O19 Mo7 O29 90.79(15) . 2_576 ?
O23 Mo7 O13 95.99(18) . . ?
O23 Mo7 O19 102.75(18) . . ?
O23 Mo7 O24 162.56(17) . . ?
O23 Mo7 O29 93.82(17) . 2_576 ?
O23 Mo7 O36 104.03(18) . . ?
O29 Mo7 O13 75.56(15) 2_576 . ?
O29 Mo7 O24 71.60(13) 2_576 . ?
O36 Mo7 O13 87.03(16) . . ?
O36 Mo7 O19 100.14(16) . . ?
O36 Mo7 O24 87.85(14) . . ?
O36 Mo7 O29 156.31(16) . 2_576 ?
O2 Mo8 O11 102.31(17) . . ?
O2 Mo8 O22 92.31(17) . . ?
O2 Mo8 O24 164.17(16) . 2_576 ?
O2 Mo8 O29 103.37(17) . . ?
O2 Mo8 O32 104.56(18) . . ?
O11 Mo8 O22 73.35(14) . . ?
O11 Mo8 O24 78.51(13) . 2_576 ?
O22 Mo8 O24 72.64(13) . 2_576 ?
O29 Mo8 O11 150.57(15) . . ?
O29 Mo8 O22 91.44(16) . . ?
O29 Mo8 O24 72.86(13) . 2_576 ?
O32 Mo8 O11 86.57(16) . . ?
O32 Mo8 O22 156.22(14) . . ?
O32 Mo8 O24 91.27(14) . 2_576 ?
O32 Mo8 O29 100.59(17) . . ?
O5 Mo9 O10 103.23(18) . . ?
O5 Mo9 O12 94.35(16) . . ?
O5 Mo9 O15 162.64(16) . 2_576 ?
O5 Mo9 O18 94.84(17) . . ?
O5 Mo9 O25 104.75(17) . . ?
O10 Mo9 O12 89.12(15) . . ?
O10 Mo9 O15 87.10(14) . 2_576 ?
O10 Mo9 O18 157.12(15) . . ?
O12 Mo9 O15 71.60(12) . 2_576 ?
O18 Mo9 O12 75.48(14) . . ?
O18 Mo9 O15 72.16(13) . 2_576 ?
O25 Mo9 O10 100.15(17) . . ?
O25 Mo9 O12 156.07(15) . . ?
O25 Mo9 O15 86.77(14) . 2_576 ?
O25 Mo9 O18 88.48(15) . . ?
O1 Mo10 O11 170.29(16) . . ?
O1 Mo10 O22 105.53(18) . . ?
O1 Mo10 O26 102.74(18) . . ?
O1 Mo10 O33 85.29(16) . . ?
O11 Mo10 O33 85.13(13) . . ?
O17 Mo10 O1 102.08(19) . . ?
O17 Mo10 O11 87.50(17) . . ?
O17 Mo10 O22 103.79(18) . . ?
O17 Mo10 O26 103.37(17) . . ?
O17 Mo10 O33 172.62(17) . . ?
O22 Mo10 O11 73.20(14) . . ?
O22 Mo10 O33 74.08(13) . . ?
O26 Mo10 O11 73.14(14) . . ?
O26 Mo10 O22 135.21(15) . . ?
O26 Mo10 O33 74.42(13) . . ?
O24 Ge1 O15 111.38(16) . . ?
O24 Ge1 O35 109.77(15) . . ?
O24 Ge1 O37 106.65(16) . . ?
O35 Ge1 O15 110.23(15) . . ?
O35 Ge1 O37 111.80(16) . . ?
O37 Ge1 O15 106.94(16) . . ?
O25 Ni1 O31 92.05(14) . . ?
O25 Ni1 O34 92.61(14) . . ?
O25 Ni1 O35 92.95(14) . 2_576 ?
O25 Ni1 O35 173.03(14) . . ?
O25 Ni1 O36 90.40(14) . . ?
O31 Ni1 O35 92.60(14) . 2_576 ?
O31 Ni1 O35 83.34(13) . . ?
O34 Ni1 O31 173.50(14) . . ?
O34 Ni1 O35 91.59(14) . . ?
O34 Ni1 O35 82.63(13) . 2_576 ?
O35 Ni1 O35 82.08(14) . 2_576 ?
O36 Ni1 O31 91.56(15) . . ?
O36 Ni1 O34 92.93(14) . . ?
O36 Ni1 O35 174.55(14) . 2_576 ?
O36 Ni1 O35 94.93(14) . . ?
O14 Ni2 O31 175.54(15) 2_576 . ?
O14 Ni2 O34 90.58(14) 2_576 2_576 ?
O14 Ni2 O35 92.30(14) 2_576 . ?
O10W Ni2 O14 89.33(15) . 2_576 ?
O10W Ni2 O31 95.10(15) . . ?
O10W Ni2 O34 94.72(15) . 2_576 ?
O10W Ni2 O35 176.99(14) . . ?
O21 Ni2 O14 90.48(14) . 2_576 ?
O21 Ni2 O10W 88.92(16) . . ?
O21 Ni2 O31 90.14(14) . . ?
O21 Ni2 O34 176.22(15) . 2_576 ?
O21 Ni2 O35 93.59(14) . . ?
O34 Ni2 O31 88.53(14) 2_576 . ?
O35 Ni2 O31 83.25(14) . . ?
O35 Ni2 O34 82.74(14) . 2_576 ?
Mo1 O8 Mo5 155.0(2) . . ?
Mo9 O10 Mo3 144.9(2) . . ?
Mo1 O11 Mo8 149.4(2) . . ?
Mo1 O11 Mo10 104.86(15) . . ?
Mo8 O11 Mo10 105.72(16) . . ?
Mo1 O12 Mo9 119.30(17) . . ?
Mo4 O13 Mo7 116.40(17) . . ?
Mo3 O14 Ni2 138.7(2) . 2_576 ?
Mo2 O15 Mo1 99.68(12) 2_576 2_576 ?
Mo9 O15 Mo1 94.26(12) 2_576 2_576 ?
Mo9 O15 Mo2 94.13(12) 2_576 2_576 ?
Ge1 O15 Mo1 120.64(16) . 2_576 ?
Ge1 O15 Mo2 120.37(16) . 2_576 ?
Ge1 O15 Mo9 121.57(17) . 2_576 ?
Ni2 O10W H10A 111.1 . . ?
Ni2 O10W H10B 108.5 . . ?
H10A O10W H10B 106.5 . . ?
Mo2 O18 Mo9 115.42(17) . . ?
Mo7 O19 Mo6 145.55(19) . . ?
Mo6 O21 Ni2 138.8(2) . . ?
Mo4 O22 Mo8 110.87(16) 2_576 . ?
Mo10 O22 Mo4 104.27(15) . 2_576 ?
Mo10 O22 Mo8 104.32(16) . . ?
Mo4 O24 Mo8 99.25(13) . 2_576 ?
Mo7 O24 Mo4 94.23(12) . . ?
Mo7 O24 Mo8 93.52(12) . 2_576 ?
Ge1 O24 Mo4 120.35(16) . . ?
Ge1 O24 Mo7 122.13(17) . . ?
Ge1 O24 Mo8 120.93(16) . 2_576 ?
Mo9 O25 Ni1 142.2(2) . . ?
Mo1 O26 Mo2 111.90(15) . . ?
Mo10 O26 Mo1 104.53(16) . . ?
Mo10 O26 Mo2 103.32(15) . . ?
Mo5 O27 Mo3 119.51(17) . . ?
Mo3 O28 Mo6 116.95(18) . 2_576 ?
Mo8 O29 Mo7 119.88(17) . 2_576 ?
Mo5 O30 Mo6 119.82(17) . 2_576 ?
Mo2 O31 Ni1 131.35(19) . . ?
Mo2 O31 Ni2 128.14(19) . . ?
Ni1 O31 Ni2 96.31(14) . . ?
Mo8 O32 Mo5 153.7(2) . . ?
Mo2 O33 Mo4 152.55(18) . 2_576 ?
Mo2 O33 Mo10 103.62(15) . . ?
Mo4 O33 Mo10 103.74(14) 2_576 . ?
Mo4 O34 Ni1 131.92(19) . . ?
Mo4 O34 Ni2 127.80(19) . 2_576 ?
Ni1 O34 Ni2 97.26(14) . 2_576 ?
Ge1 O35 Ni1 120.37(17) . . ?
Ge1 O35 Ni1 120.21(17) . 2_576 ?
Ge1 O35 Ni2 119.37(18) . . ?
Ni1 O35 Ni1 97.93(14) . 2_576 ?
Ni2 O35 Ni1 96.77(13) . . ?
Ni2 O35 Ni1 96.90(14) . 2_576 ?
Mo7 O36 Ni1 139.8(2) . . ?
Mo3 O37 Mo5 92.07(12) 2_576 2_576 ?
Mo6 O37 Mo3 91.71(12) . 2_576 ?
Mo6 O37 Mo5 93.01(12) . 2_576 ?
Ge1 O37 Mo3 120.92(16) . 2_576 ?
Ge1 O37 Mo5 128.70(17) . 2_576 ?
Ge1 O37 Mo6 121.03(16) . . ?
N7 Ni3 N7 180.0(2) 2_677 . ?
N8 Ni3 N7 90.48(17) 2_677 2_677 ?
N8 Ni3 N7 90.48(17) . . ?
N8 Ni3 N7 89.52(17) 2_677 . ?
N8 Ni3 N7 89.52(17) . 2_677 ?
N8 Ni3 N8 180.0 2_677 . ?
N11 Ni3 N7 90.73(17) . . ?
N11 Ni3 N7 90.73(17) 2_677 2_677 ?
N11 Ni3 N7 89.27(17) . 2_677 ?
N11 Ni3 N7 89.27(17) 2_677 . ?
N11 Ni3 N8 89.55(17) . . ?
N11 Ni3 N8 90.45(17) . 2_677 ?
N11 Ni3 N8 89.55(17) 2_677 2_677 ?
N11 Ni3 N8 90.45(17) 2_677 . ?
N11 Ni3 N11 180.0(3) . 2_677 ?
O1W Ni4 O2W 83.38(18) . . ?
O1W Ni4 O3W 85.09(19) . . ?
O1W Ni4 N6 95.86(19) . . ?
O1W Ni4 N12 92.24(19) . . ?
O2W Ni4 O3W 89.5(2) . . ?
N6 Ni4 O2W 178.00(19) . . ?
N6 Ni4 O3W 88.60(19) . . ?
N6 Ni4 N12 90.19(19) . . ?
N9 Ni4 O1W 170.44(18) . . ?
N9 Ni4 O2W 89.70(17) . . ?
N9 Ni4 O3W 88.26(18) . . ?
N9 Ni4 N6 90.84(17) . . ?
N9 Ni4 N12 94.56(17) . . ?
N12 Ni4 O2W 91.69(19) . . ?
N12 Ni4 O3W 176.95(18) . . ?
Ni4 O1W H1WA 110.5 . . ?
Ni4 O1W H1WB 110.8 . . ?
H1WA O1W H1WB 109.0 . . ?
Ni4 O2W H2WA 124.8 . . ?
Ni4 O2W H2WB 116.5 . . ?
H2WA O2W H2WB 111.2 . . ?
Ni4 O3W H3WA 111.5 . . ?
Ni4 O3W H3WB 111.1 . . ?
H3WA O3W H3WB 102.4 . . ?
C2 N1 N4 127.7(6) . . ?
C2 N1 C3 107.2(5) . . ?
C3 N1 N4 125.1(5) . . ?
H2A N2 H2B 120.0 . . ?
N5 N2 H2A 120.0 . . ?
N5 N2 H2B 120.0 . . ?
H3A N3 H3B 120.0 . . ?
N10 N3 H3A 120.0 . . ?
N10 N3 H3B 120.0 . . ?
N1 N4 H4A 120.0 . . ?
N1 N4 H4B 120.0 . . ?
H4A N4 H4B 120.0 . . ?
C1 N5 N2 128.2(5) . . ?
C1 N5 C4 105.2(5) . . ?
C4 N5 N2 126.7(5) . . ?
N8 N6 Ni4 122.2(3) . . ?
C3 N6 Ni4 131.0(4) . . ?
C3 N6 N8 106.8(5) . . ?
N9 N7 Ni3 122.5(3) . . ?
C6 N7 Ni3 130.0(4) . . ?
C6 N7 N9 107.2(4) . . ?
N6 N8 Ni3 126.2(3) . . ?
C2 N8 Ni3 126.0(4) . . ?
C2 N8 N6 107.7(5) . . ?
N7 N9 Ni4 126.8(3) . . ?
C5 N9 Ni4 125.5(4) . . ?
C5 N9 N7 107.7(4) . . ?
C5 N10 N3 128.6(5) . . ?
C5 N10 C6 106.1(4) . . ?
C6 N10 N3 125.4(5) . . ?
N12 N11 Ni3 127.0(3) . . ?
C4 N11 Ni3 123.6(4) . . ?
C4 N11 N12 107.6(4) . . ?
N11 N12 Ni4 121.9(3) . . ?
C1 N12 Ni4 131.0(4) . . ?
C1 N12 N11 106.4(5) . . ?
N5 C1 H1 124.3 . . ?
N12 C1 N5 111.3(5) . . ?
N12 C1 H1 124.3 . . ?
N1 C2 H2 125.6 . . ?
N8 C2 N1 108.8(5) . . ?
N8 C2 H2 125.6 . . ?
N1 C3 H3 125.3 . . ?
N6 C3 N1 109.5(5) . . ?
N6 C3 H3 125.3 . . ?
N5 C4 H4 125.3 . . ?
N11 C4 N5 109.4(5) . . ?
N11 C4 H4 125.3 . . ?
N9 C5 N10 109.7(5) . . ?
N9 C5 H5 125.1 . . ?
N10 C5 H5 125.1 . . ?
N7 C6 N10 109.3(5) . . ?
N7 C6 H6 125.4 . . ?
N10 C6 H6 125.4 . . ?
H4WA O4W H4WB 111.7 . . ?
H5WA O5W H5WB 108.8 . . ?
H6WA O6W H6WB 131.1 . . ?
H7WA O7W H7WB 110.7 . . ?
H7WC O7WA H7WD 113.1 . . ?
H8WA O8W H8WB 104.6 . . ?
H9WA O9W H9WB 97.4 . . ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
_geom_hbond_publ_flag
O1W H1WB O1 0.85 1.86 2.673(6) 158.5 2_566 yes
O3W H3WB O7W 0.89 1.89 2.672(9) 146.1 . yes
O4W H4WA O10W 0.85 1.83 2.603(6) 150.7 . yes
O4W H4WB O30 0.85 1.96 2.724(6) 148.9 1_556 yes
O5W H5WB O20 0.85 2.08 2.893(8) 161.3 2_566 yes
O7W H7WB O5 0.84 2.02 2.841(9) 167.1 . yes
O7WA H7WC O13 0.85 2.07 2.871(15) 156.9 2_676 yes
O7WA H7WD O5 0.85 1.99 2.835(15) 176.6 . yes
O8W H8WA O5W 0.81 2.11 2.833(12) 148.8 2_566 yes
O8W H8WB O9W 0.85 2.03 2.81(2) 152.8 . yes

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O2 Mo8 O29 Mo7 176.9(2) . . . 2_576 ?
O2 Mo8 O32 Mo5 -131.4(4) . . . . ?
O3 Mo5 O27 Mo3 169.2(2) . . . . ?
O3 Mo5 O30 Mo6 -170.1(2) . . . 2_576 ?
O4 Mo6 O21 Ni2 149.5(3) . . . . ?
O5 Mo9 O10 Mo3 -126.7(3) . . . . ?
O5 Mo9 O25 Ni1 -149.1(3) . . . . ?
O6 Mo4 O13 Mo7 -179.70(19) . . . . ?
O6 Mo4 O34 Ni1 150.0(2) . . . . ?
O6 Mo4 O34 Ni2 -54.3(3) . . . 2_576 ?
O7 Mo1 O8 Mo5 131.6(5) . . . . ?
O7 Mo1 O12 Mo9 -175.7(2) . . . . ?
O8 Mo1 O12 Mo9 76.0(2) . . . . ?
O8 Mo5 O27 Mo3 -89.8(2) . . . . ?
O8 Mo5 O30 Mo6 38.0(5) . . . 2_576 ?
O9 Mo3 O14 Ni2 146.7(3) . . . 2_576 ?
O10 Mo3 O14 Ni2 -113.7(3) . . . 2_576 ?
O10 Mo9 O25 Ni1 104.1(3) . . . . ?
O11 Mo1 O8 Mo5 30.4(5) . . . . ?
O11 Mo1 O12 Mo9 -25.0(4) . . . . ?
O11 Mo8 O29 Mo7 26.7(5) . . . 2_576 ?
O11 Mo8 O32 Mo5 -29.6(5) . . . . ?
O12 Mo1 O8 Mo5 -120.9(5) . . . . ?
O12 Mo9 O10 Mo3 139.1(3) . . . . ?
O12 Mo9 O25 Ni1 -7.3(6) . . . . ?
O13 Mo4 O34 Ni1 43.3(3) . . . . ?
O13 Mo4 O34 Ni2 -161.0(2) . . . 2_576 ?
O13 Mo7 O19 Mo6 84.1(5) . . . . ?
O13 Mo7 O36 Ni1 -57.1(3) . . . . ?
O15 Mo1 O8 Mo5 -48.0(5) 2_576 . . . ?
O15 Mo1 O12 Mo9 -12.00(17) 2_576 . . . ?
O15 Mo2 O18 Mo9 15.05(15) 2_576 . . . ?
O15 Mo2 O31 Ni1 -29.8(2) 2_576 . . . ?
O15 Mo2 O31 Ni2 121.5(2) 2_576 . . . ?
O15 Mo9 O10 Mo3 67.5(3) 2_576 . . . ?
O15 Mo9 O25 Ni1 17.7(3) 2_576 . . . ?
O15 Ge1 O24 Mo4 -63.9(2) . . . . ?
O15 Ge1 O24 Mo7 178.17(17) . . . . ?
O15 Ge1 O24 Mo8 60.7(2) . . . 2_576 ?
O15 Ge1 O35 Ni1 0.7(2) . . . 2_576 ?
O15 Ge1 O35 Ni1 122.42(19) . . . . ?
O15 Ge1 O35 Ni2 -118.47(19) . . . . ?
O15 Ge1 O37 Mo3 63.7(2) . . . 2_576 ?
O15 Ge1 O37 Mo5 -58.5(2) . . . 2_576 ?
O15 Ge1 O37 Mo6 177.37(16) . . . . ?
O18 Mo2 O31 Ni1 45.3(3) . . . . ?
O18 Mo2 O31 Ni2 -163.5(2) . . . . ?
O18 Mo9 O10 Mo3 92.1(5) . . . . ?
O18 Mo9 O25 Ni1 -54.5(3) . . . . ?
O19 Mo6 O21 Ni2 -110.2(3) . . . . ?
O19 Mo7 O36 Ni1 101.4(3) . . . . ?
O20 Mo2 O18 Mo9 179.35(18) . . . . ?
O20 Mo2 O31 Ni1 149.7(2) . . . . ?
O20 Mo2 O31 Ni2 -59.0(3) . . . . ?
O22 Mo4 O13 Mo7 87.13(19) 2_576 . . . ?
O22 Mo4 O34 Ni1 -72.3(5) 2_576 . . . ?
O22 Mo4 O34 Ni2 83.4(5) 2_576 . . 2_576 ?
O22 Mo8 O29 Mo7 84.1(2) . . . 2_576 ?
O22 Mo8 O32 Mo5 2.5(7) . . . . ?
O23 Mo7 O19 Mo6 -130.1(4) . . . . ?
O23 Mo7 O36 Ni1 -152.6(3) . . . . ?
O24 Mo4 O13 Mo7 13.71(16) . . . . ?
O24 Mo4 O34 Ni1 -31.6(2) . . . . ?
O24 Mo4 O34 Ni2 124.0(2) . . . 2_576 ?
O24 Mo7 O19 Mo6 64.3(3) . . . . ?
O24 Mo7 O36 Ni1 14.5(3) . . . . ?
O24 Mo8 O29 Mo7 12.81(18) 2_576 . . 2_576 ?
O24 Mo8 O32 Mo5 48.9(5) 2_576 . . . ?
O24 Ge1 O15 Mo1 -60.8(2) . . . 2_576 ?
O24 Ge1 O15 Mo2 64.2(2) . . . 2_576 ?
O24 Ge1 O15 Mo9 -178.55(17) . . . 2_576 ?
O24 Ge1 O35 Ni1 -122.36(19) . . . 2_576 ?
O24 Ge1 O35 Ni1 -0.6(2) . . . . ?
O24 Ge1 O35 Ni2 118.49(19) . . . . ?
O24 Ge1 O37 Mo3 -177.00(16) . . . 2_576 ?
O24 Ge1 O37 Mo5 60.7(2) . . . 2_576 ?
O24 Ge1 O37 Mo6 -63.4(2) . . . . ?
O25 Mo9 O10 Mo3 -18.7(4) . . . . ?
O26 Mo1 O8 Mo5 -3.6(8) . . . . ?
O26 Mo1 O12 Mo9 -83.1(2) . . . . ?
O26 Mo2 O18 Mo9 88.05(18) . . . . ?
O26 Mo2 O31 Ni1 -69.3(5) . . . . ?
O26 Mo2 O31 Ni2 82.0(5) . . . . ?
O27 Mo3 O14 Ni2 -33.8(7) . . . 2_576 ?
O27 Mo5 O30 Mo6 -64.3(2) . . . 2_576 ?
O28 Mo3 O14 Ni2 44.4(3) . . . 2_576 ?
O28 Mo6 O21 Ni2 48.8(3) 2_576 . . . ?
O29 Mo7 O19 Mo6 135.8(3) 2_576 . . . ?
O29 Mo7 O36 Ni1 -14.8(6) 2_576 . . . ?
O29 Mo8 O32 Mo5 121.7(4) . . . . ?
O30 Mo5 O27 Mo3 65.5(2) . . . . ?
O30 Mo6 O21 Ni2 -26.5(7) 2_576 . . . ?
O31 Mo2 O18 Mo9 -72.9(2) . . . . ?
O32 Mo5 O27 Mo3 -29.2(5) . . . . ?
O32 Mo5 O30 Mo6 92.4(2) . . . 2_576 ?
O32 Mo8 O29 Mo7 -75.2(2) . . . 2_576 ?
O33 Mo2 O18 Mo9 33.9(4) . . . . ?
O33 Mo2 O31 Ni1 -108.7(3) . . . . ?
O33 Mo2 O31 Ni2 42.6(2) . . . . ?
O33 Mo4 O13 Mo7 30.9(4) 2_576 . . . ?
O33 Mo4 O34 Ni1 -110.6(3) 2_576 . . . ?
O33 Mo4 O34 Ni2 45.1(2) 2_576 . . 2_576 ?
O34 Mo4 O13 Mo7 -73.2(2) . . . . ?
O35 Ge1 O15 Mo1 177.08(16) . . . 2_576 ?
O35 Ge1 O15 Mo2 -57.9(2) . . . 2_576 ?
O35 Ge1 O15 Mo9 59.4(2) . . . 2_576 ?
O35 Ge1 O24 Mo4 58.5(2) . . . . ?
O35 Ge1 O24 Mo7 -59.5(2) . . . . ?
O35 Ge1 O24 Mo8 -176.90(17) . . . 2_576 ?
O35 Ge1 O37 Mo3 -57.0(2) . . . 2_576 ?
O35 Ge1 O37 Mo5 -179.27(18) . . . 2_576 ?
O35 Ge1 O37 Mo6 56.6(2) . . . . ?
O36 Mo7 O19 Mo6 -23.1(4) . . . . ?
O37 Mo3 O14 Ni2 -29.6(3) 2_576 . . 2_576 ?
O37 Mo5 O27 Mo3 -5.56(17) 2_576 . . . ?
O37 Mo5 O30 Mo6 8.04(17) 2_576 . . 2_576 ?
O37 Mo6 O21 Ni2 -25.0(3) . . . . ?
O37 Ge1 O15 Mo1 55.3(2) . . . 2_576 ?
O37 Ge1 O15 Mo2 -179.65(16) . . . 2_576 ?
O37 Ge1 O15 Mo9 -62.4(2) . . . 2_576 ?
O37 Ge1 O24 Mo4 179.78(16) . . . . ?
O37 Ge1 O24 Mo7 61.8(2) . . . . ?
O37 Ge1 O24 Mo8 -55.6(2) . . . 2_576 ?
O37 Ge1 O35 Ni1 119.49(19) . . . 2_576 ?
O37 Ge1 O35 Ni1 -118.77(19) . . . . ?
O37 Ge1 O35 Ni2 0.3(2) . . . . ?
Ni3 N7 N9 Ni4 5.6(5) . . . . ?
Ni3 N7 N9 C5 -173.8(3) . . . . ?
Ni3 N7 C6 N10 172.3(3) . . . . ?
Ni3 N8 C2 N1 177.5(3) . . . . ?
Ni3 N11 N12 Ni4 -7.4(6) . . . . ?
Ni3 N11 N12 C1 164.0(4) . . . . ?
Ni3 N11 C4 N5 -164.2(3) . . . . ?
Ni4 N6 N8 Ni3 0.6(6) . . . . ?
Ni4 N6 N8 C2 177.9(4) . . . . ?
Ni4 N6 C3 N1 -177.3(4) . . . . ?
Ni4 N9 C5 N10 -178.9(3) . . . . ?
Ni4 N12 C1 N5 170.3(4) . . . . ?
N2 N5 C1 N12 -179.5(5) . . . . ?
N2 N5 C4 N11 179.0(5) . . . . ?
N3 N10 C5 N9 178.8(5) . . . . ?
N3 N10 C6 N7 -178.4(5) . . . . ?
N4 N1 C2 N8 -179.6(5) . . . . ?
N4 N1 C3 N6 178.9(5) . . . . ?
N6 N8 C2 N1 0.2(6) . . . . ?
N7 N9 C5 N10 0.6(6) . . . . ?
N8 N6 C3 N1 1.4(6) . . . . ?
N9 N7 C6 N10 -1.6(6) . . . . ?
N11 N12 C1 N5 0.0(7) . . . . ?
N12 N11 C4 N5 1.1(6) . . . . ?
C1 N5 C4 N11 -1.1(6) . . . . ?
C2 N1 C3 N6 -1.3(7) . . . . ?
C3 N1 C2 N8 0.6(6) . . . . ?
C3 N6 N8 Ni3 -178.3(4) . . . . ?
C3 N6 N8 C2 -1.0(6) . . . . ?
C4 N5 C1 N12 0.7(7) . . . . ?
C4 N11 N12 Ni4 -172.1(4) . . . . ?
C4 N11 N12 C1 -0.7(6) . . . . ?
C5 N10 C6 N7 1.9(6) . . . . ?
C6 N7 N9 Ni4 -179.9(3) . . . . ?
C6 N7 N9 C5 0.7(5) . . . . ?
C6 N10 C5 N9 -1.5(6) . . . . ?

_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1_CCDC1
_database_code_depnum_ccdc_archive 'CCDC 1961646'
loop_
_audit_author_name
_audit_author_address
'hui xu'
;Jilin University
China
;
_audit_update_record             
;
2019-10-28 deposited with the CCDC.	2019-12-17 downloaded from the CCDC.
;
_audit_creation_date             2019-10-21
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2018/3
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         
'Co4 Ge2 H4 Mo20 O74, C12 H36 Co3 N24 O6, 11(H2 O)'
_chemical_formula_sum            'C12 H62 Co7 Ge2 Mo20 N24 O91'
_chemical_formula_weight         4475.39
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0181 0.0091 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co -2.3653 3.6143 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge -1.0885 0.8855 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -0.0483 2.7339 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0311 0.0180 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0492 0.0322 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   13.9114(12)
_cell_length_b                   14.1874(12)
_cell_length_c                   14.6356(13)
_cell_angle_alpha                110.550(4)
_cell_angle_beta                 98.559(4)
_cell_angle_gamma                112.651(4)
_cell_volume                     2357.5(4)
_cell_formula_units_Z            1
_cell_measurement_reflns_used    9922
_cell_measurement_temperature    173(2)
_cell_measurement_theta_max      66.767
_cell_measurement_theta_min      3.414
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    32.285
_exptl_absorpt_correction_T_max  0.002
_exptl_absorpt_correction_T_min  0.001
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Krause et al., 2015) was used for absorption correction.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            'orange yellow'
_exptl_crystal_colour_primary    'orange yellow'
_exptl_crystal_density_diffrn    3.152
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             2123
_exptl_crystal_size_max          0.24
_exptl_crystal_size_mid          0.22
_exptl_crystal_size_min          0.2
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0455
_diffrn_reflns_av_unetI/netI     0.0418
_diffrn_reflns_Laue_measured_fraction_full 0.989
_diffrn_reflns_Laue_measured_fraction_max 0.989
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            31585
_diffrn_reflns_point_group_measured_fraction_full 0.989
_diffrn_reflns_point_group_measured_fraction_max 0.989
_diffrn_reflns_theta_full        66.853
_diffrn_reflns_theta_max         66.853
_diffrn_reflns_theta_min         3.415
_diffrn_ambient_temperature      173.0
_diffrn_detector_area_resol_mean 7.9
_diffrn_detector_type            'Bruker APEX II'
_diffrn_measured_fraction_theta_full 0.989
_diffrn_measured_fraction_theta_max 0.989
_diffrn_measurement_device       'three-circle diffractometer'
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54178
_diffrn_source                   ?
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                7085
_reflns_number_total             8380
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT V8.38A (?, 2016)'
_computing_data_collection       'APEX3 Ver. 2016.5-0 (Bruker-AXS, 2016)'
_computing_data_reduction        'SAINT V8.38A (?, 2016)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_refine_diff_density_max         0.770
_refine_diff_density_min         -1.077
_refine_diff_density_rms         0.196
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.050
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     732
_refine_ls_number_reflns         8291
_refine_ls_number_restraints     18
_refine_ls_R_factor_all          0.0405
_refine_ls_R_factor_gt           0.0310
_refine_ls_restrained_S_all      1.053
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0253P)²+9.8766P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0675
_refine_ls_wR_factor_ref         0.0716
_refine_special_details          ?
_olex2_refinement_description    
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All N(H,H) groups
 At 1.5 times of:
  All O(H,H) groups
2. Uiso/Uaniso restraints and constraints
Uanis(O10W) \\sim Ueq, Uanis(N4) \\sim Ueq: with sigma of 0.005 and sigma for
terminal atoms of 0.01
Uanis(O36) \\sim Ueq: with sigma of 0.001 and sigma for terminal atoms of 0.002
3. Others
 Sof(O7WA)=Sof(H7WC)=Sof(H7WD)=1-FVAR(1)
 Sof(O7W)=Sof(H7WA)=Sof(H7WB)=FVAR(1)
 Sof(O9WA)=Sof(H9WC)=Sof(H9WD)=1-FVAR(2)
 Sof(O9W)=Sof(H9WA)=Sof(H9WB)=FVAR(2)
 Fixed Sof: O10W(0.5) H10A(0.5) H10B(0.5)
4.a Riding coordinates:
 O1W(H1WA,H1WB), O5W(H5WA,H5WB), O6W(H6WA,H6WB), O7W(H7WA,H7WB), O7WA(H7WC,
 H7WD), O8W(H8WA,H8WB), O9W(H9WA,H9WB), O9WA(H9WC,H9WD), O10W(H10A,H10B)
4.b Rotating group:
 O2W(H2WA,H2WB), O3W(H3WA,H3WB), O4W(H4WA,H4WB)
4.c Aromatic/amide H refined with riding coordinates:
 C3(H3), C5(H5), C1(H1), C2(H2), C4(H4), C6(H6)
4.d X=CH2 refined with riding coordinates:
 N4(H4A,H4B), N8(H8A,H8B), N12(H12A,H12B)
;
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.31728(4) -0.80508(4) 0.14492(3) 0.00870(10) Uani 1 1 d . . . . .
Mo2 Mo 0.59903(4) -0.66650(4) 0.48872(3) 0.00956(10) Uani 1 1 d . . . . .
Mo3 Mo 0.50012(4) -0.70500(3) 0.03584(3) 0.00806(10) Uani 1 1 d . . . . .
Mo4 Mo 0.77857(4) -0.70247(4) 0.10975(3) 0.00866(10) Uani 1 1 d . . . . .
Mo5 Mo 0.54345(4) -0.55191(4) 0.30476(3) 0.00941(10) Uani 1 1 d . . . . .
Mo6 Mo 0.82448(4) -0.79990(4) 0.27989(3) 0.00961(10) Uani 1 1 d . . . . .
Mo7 Mo 0.81704(4) -0.54993(4) 0.37680(3) 0.00976(10) Uani 1 1 d . . . . .
Mo8 Mo 0.61202(4) -0.91502(4) 0.38839(3) 0.00975(10) Uani 1 1 d . . . . .
Mo9 Mo 0.37302(4) -0.91801(4) 0.32603(3) 0.00950(10) Uani 1 1 d . . . . .
Mo10 Mo 0.73318(4) -0.48204(4) 0.19860(4) 0.01219(11) Uani 1 1 d . . . . .
Ge1 Ge 0.56582(5) -0.81233(5) 0.20750(5) 0.00577(13) Uani 1 1 d . . . . .
Co1 Co 0.43426(8) -1.09448(7) 0.12609(7) 0.0102(2) Uani 1 1 d . . . . .
Co2 Co 0.61620(7) -0.99871(7) 0.03170(7) 0.00890(19) Uani 1 1 d . . . . .
O1 O 0.4722(3) -0.8483(3) -0.0416(3) 0.0136(9) Uani 1 1 d . . . . .
O1W O 0.3523(4) -1.2438(3) 0.1377(3) 0.0214(10) Uani 1 1 d . . . . .
H1WA H 0.367261 -1.229705 0.201338 0.032 Uiso 1 1 d R . . . .
H1WB H 0.293311 -1.299835 0.097678 0.032 Uiso 1 1 d R . . . .
O2 O 0.6565(3) -0.6638(3) 0.0925(3) 0.0120(8) Uani 1 1 d . . . . .
O3 O 0.5719(3) -0.5379(3) 0.1692(3) 0.0131(8) Uani 1 1 d . . . . .
O4 O 0.6834(3) -0.8467(3) 0.0171(3) 0.0117(8) Uani 1 1 d . . . . .
O5 O 0.3950(3) -0.6278(3) 0.2402(3) 0.0136(9) Uani 1 1 d . . . . .
O6 O 0.4554(3) -0.7598(3) 0.4602(3) 0.0134(8) Uani 1 1 d . . . . .
O7 O 0.8986(3) -0.6236(3) 0.3720(3) 0.0141(9) Uani 1 1 d . . . . .
O8 O 0.6897(3) -0.5388(3) 0.3126(3) 0.0134(9) Uani 1 1 d . . . . .
O9 O 0.5116(3) -0.9489(3) 0.1038(3) 0.0079(8) Uani 1 1 d . . . . .
O10 O 0.6541(3) -0.7584(3) 0.5098(3) 0.0112(8) Uani 1 1 d . . . . .
O11 O 0.8383(3) -0.5348(3) 0.2378(3) 0.0135(9) Uani 1 1 d . . . . .
O12 O 0.9401(3) -0.8067(4) 0.3200(3) 0.0214(10) Uani 1 1 d . . . . .
O13 O 0.3638(3) -0.7320(3) 0.0462(3) 0.0132(8) Uani 1 1 d . . . . .
O14 O 0.5462(3) -0.8207(3) 0.3203(3) 0.0084(8) Uani 1 1 d . . . . .
O15 O 0.7411(3) -0.9304(3) 0.1681(3) 0.0147(9) Uani 1 1 d . . . . .
O16 O 0.3465(3) -1.0261(3) 0.2061(3) 0.0142(9) Uani 1 1 d . . . . .
O17 O 0.4985(3) -0.7389(3) 0.1792(3) 0.0077(8) Uani 1 1 d . . . . .
O18 O 0.3026(3) -0.9328(3) 0.0533(3) 0.0137(9) Uani 1 1 d . . . . .
O19 O 0.7518(3) -0.8267(3) 0.3717(3) 0.0135(8) Uani 1 1 d . . . . .
O20 O 0.8765(3) -0.7280(3) 0.1813(3) 0.0136(9) Uani 1 1 d . . . . .
O21 O 0.5505(3) -0.5949(3) 0.4070(3) 0.0157(9) Uani 1 1 d . . . . .
O22 O 0.5582(3) -1.0276(3) 0.2640(3) 0.0157(9) Uani 1 1 d . . . . .
O23 O 0.7413(3) -0.5919(3) 0.4580(3) 0.0141(9) Uani 1 1 d . . . . .
O24 O 0.3337(3) -0.8280(3) 0.2615(3) 0.0137(8) Uani 1 1 d . . . . .
O25 O 0.2577(3) -0.9698(4) 0.3570(3) 0.0205(10) Uani 1 1 d . . . . .
O26 O 0.5065(4) -0.6457(3) -0.0466(3) 0.0210(10) Uani 1 1 d . . . . .
O27 O 0.4668(3) -0.9519(3) 0.4034(3) 0.0120(8) Uani 1 1 d . . . . .
O28 O 0.8470(3) -0.6464(3) 0.0393(3) 0.0214(10) Uani 1 1 d . . . . .
O29 O 0.6370(3) -0.5673(3) 0.6106(3) 0.0178(9) Uani 1 1 d . . . . .
O30 O 0.1879(3) -0.8179(4) 0.1165(3) 0.0211(10) Uani 1 1 d . . . . .
O31 O 0.7879(4) -0.3460(3) 0.2924(3) 0.0211(10) Uani 1 1 d . . . . .
O32 O 0.5732(4) -0.4140(3) 0.3651(3) 0.0196(10) Uani 1 1 d . . . . .
O33 O 0.6594(3) -0.9632(3) 0.4657(3) 0.0172(9) Uani 1 1 d . . . . .
O34 O 0.7545(4) -0.4611(4) 0.0920(4) 0.0279(11) Uani 1 1 d . . . . .
O35 O 0.9107(3) -0.4113(3) 0.4535(3) 0.0200(10) Uani 1 1 d . . . . .
O36 O 0.7084(3) -0.7369(3) 0.2345(3) 0.0070(8) Uani 1 1 d . U . . .
Co3 Co 1.05557(8) 0.10760(8) 0.78985(7) 0.0164(2) Uani 1 1 d . . . . .
Co4 Co 1.000000 0.000000 0.500000 0.0107(3) Uani 1 2 d S T P . .
O2W O 0.9339(5) 0.1017(5) 0.8638(4) 0.0418(14) Uani 1 1 d . . . . .
H2WA H 0.878900 0.097557 0.826443 0.063 Uiso 1 1 d GR . . . .
H2WB H 0.964740 0.136486 0.930293 0.063 Uiso 1 1 d GR . . . .
O3W O 1.1158(4) 0.0393(4) 0.8799(4) 0.0328(12) Uani 1 1 d . . . . .
H3WA H 1.145516 0.088748 0.945505 0.049 Uiso 1 1 d GR . . . .
H3WB H 1.171319 0.029951 0.864836 0.049 Uiso 1 1 d GR . . . .
O4W O 1.1640(5) 0.2630(4) 0.9196(4) 0.0446(15) Uani 1 1 d . . . . .
H4WA H 1.135403 0.309110 0.933261 0.067 Uiso 1 1 d GR . . . .
H4WB H 1.221734 0.299542 0.905730 0.067 Uiso 1 1 d GR . . . .
N3 N 0.8197(4) -0.2348(4) 0.6063(4) 0.0135(11) Uani 1 1 d . . . . .
N10 N 0.9704(4) 0.1330(4) 0.5956(4) 0.0162(11) Uani 1 1 d . . . . .
N5 N 0.8436(4) -0.0764(4) 0.3878(4) 0.0150(11) Uani 1 1 d . . . . .
N2 N 0.9258(4) -0.1024(4) 0.5737(4) 0.0133(10) Uani 1 1 d . . . . .
N9 N 0.9892(4) 0.1729(4) 0.7006(4) 0.0168(11) Uani 1 1 d . . . . .
N7 N 0.6669(4) -0.1799(4) 0.3171(4) 0.0198(12) Uani 1 1 d . . . . .
N6 N 0.8184(4) -0.1231(4) 0.2810(4) 0.0174(11) Uani 1 1 d . . . . .
N1 N 0.9460(4) -0.0580(4) 0.6788(4) 0.0111(10) Uani 1 1 d . . . . .
N11 N 0.9288(4) 0.2708(4) 0.6471(5) 0.0238(13) Uani 1 1 d . . . . .
N4 N 0.7386(5) -0.3413(4) 0.5920(5) 0.0332(15) Uani 1 1 d . U . . .
H4A H 0.703303 -0.398532 0.529539 0.040 Uiso 1 1 calc R . . . .
H4B H 0.723406 -0.350410 0.645508 0.040 Uiso 1 1 calc R . . . .
N8 N 0.5539(4) -0.2379(5) 0.3054(5) 0.0309(14) Uani 1 1 d . . . . .
H8A H 0.504657 -0.283204 0.243252 0.037 Uiso 1 1 calc R . . . .
H8B H 0.532773 -0.228497 0.360298 0.037 Uiso 1 1 calc R . . . .
N12 N 0.8964(5) 0.3543(5) 0.6506(6) 0.0360(16) Uani 1 1 d . . . . .
H12A H 0.897291 0.400978 0.709630 0.043 Uiso 1 1 calc R . . . .
H12B H 0.875315 0.359720 0.593752 0.043 Uiso 1 1 calc R . . . .
C3 C 0.7508(5) -0.1115(5) 0.4060(5) 0.0211(14) Uani 1 1 d . . . . .
H3 H 0.743631 -0.091580 0.472835 0.025 Uiso 1 1 calc R . . . .
C5 C 0.9624(5) 0.2546(5) 0.7284(5) 0.0231(15) Uani 1 1 d . . . . .
H5 H 0.966076 0.296790 0.796727 0.028 Uiso 1 1 calc R . . . .
C1 C 0.8816(5) -0.1403(5) 0.6960(5) 0.0149(13) Uani 1 1 d . . . . .
H1 H 0.878896 -0.134261 0.762207 0.018 Uiso 1 1 calc R . . . .
C2 C 0.8499(5) -0.2105(5) 0.5315(5) 0.0168(13) Uani 1 1 d . . . . .
H2 H 0.821556 -0.262323 0.460130 0.020 Uiso 1 1 calc R . . . .
C4 C 0.7115(5) -0.1853(5) 0.2417(5) 0.0256(15) Uani 1 1 d . . . . .
H4 H 0.671075 -0.228341 0.169940 0.031 Uiso 1 1 calc R . . . .
C6 C 0.9351(5) 0.1937(5) 0.5651(5) 0.0194(14) Uani 1 1 d . . . . .
H6 H 0.916819 0.184973 0.496383 0.023 Uiso 1 1 calc R . . . .
O5W O 0.6493(6) 0.1912(5) 0.6740(4) 0.065(2) Uani 1 1 d . . . . .
H5WA H 0.682024 0.229114 0.646781 0.098 Uiso 1 1 d R . . . .
H5WB H 0.651454 0.132054 0.626611 0.098 Uiso 1 1 d R . . . .
O6W O 0.3673(6) -0.4801(6) 0.1405(6) 0.073(2) Uani 1 1 d . . . . .
H6WA H 0.304172 -0.493280 0.146505 0.110 Uiso 1 1 d R . . . .
H6WB H 0.381262 -0.514600 0.172925 0.110 Uiso 1 1 d R . . . .
O7W O 0.9681(9) 0.1407(11) 1.0617(8) 0.032(4) Uani 0.49(2) 1 d . . . A 1
H7WA H 0.942130 0.087424 1.068030 0.048 Uiso 0.49(2) 1 d R . . A 1
H7WB H 1.036360 0.177854 1.093300 0.048 Uiso 0.49(2) 1 d R . . A 1
O7WA O 1.0190(14) 0.239(2) 1.0695(10) 0.083(9) Uani 0.51(2) 1 d . . . A 2
H7WC H 0.973795 0.227842 1.102516 0.124 Uiso 0.51(2) 1 d R . . A 2
H7WD H 1.076045 0.232352 1.095906 0.124 Uiso 0.51(2) 1 d R . . A 2
O8W O 0.8854(6) -0.4156(8) 0.6916(9) 0.136(5) Uani 1 1 d . . . . .
H8WA H 0.953918 -0.392089 0.700869 0.204 Uiso 1 1 d R . . . .
H8WB H 0.849628 -0.464029 0.626559 0.204 Uiso 1 1 d R . . . .
O9W O 0.828(3) 0.478(2) 0.832(3) 0.089(10) Uani 0.48(7) 1 d . . . B 1
H9WA H 0.872783 0.549844 0.851899 0.133 Uiso 0.48(7) 1 d R . . B 1
H9WB H 0.852613 0.463724 0.881129 0.133 Uiso 0.48(7) 1 d R . . B 1
O9WA O 0.843(4) 0.543(10) 0.862(6) 0.26(3) Uani 0.52(7) 1 d . . . B 2
H9WC H 0.877567 0.504091 0.866159 0.396 Uiso 0.52(7) 1 d R . . B 2
H9WD H 0.863127 0.567881 0.818319 0.396 Uiso 0.52(7) 1 d R . . B 2
O10W O 0.9964(17) 0.4413(15) 0.9490(14) 0.125(7) Uani 0.5 1 d . U . C -1
H10A H 0.937376 0.437445 0.914319 0.187 Uiso 0.5 1 d R . . C -1
H10B H 0.980296 0.429065 1.000369 0.187 Uiso 0.5 1 d R . . C -1


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O5 2.106(4) . ?
Mo1 O13 2.096(4) . ?
Mo1 O17 2.226(4) . ?
Mo1 O18 1.746(4) . ?
Mo1 O24 1.844(4) . ?
Mo1 O30 1.709(4) . ?
Mo2 O6 1.802(4) . ?
Mo2 O10 1.834(4) . ?
Mo2 O14 2.416(4) . ?
Mo2 O21 2.015(4) . ?
Mo2 O23 2.055(4) . ?
Mo2 O29 1.681(4) . ?
Mo3 O1 1.793(4) . ?
Mo3 O2 1.976(4) . ?
Mo3 O3 2.185(4) . ?
Mo3 O13 1.826(4) . ?
Mo3 O17 2.313(4) . ?
Mo3 O26 1.691(4) . ?
Mo4 O2 1.984(4) . ?
Mo4 O4 1.791(4) . ?
Mo4 O11 2.178(4) . ?
Mo4 O20 1.818(4) . ?
Mo4 O28 1.700(4) . ?
Mo4 O36 2.305(4) . ?
Mo5 O3 2.141(4) . ?
Mo5 O5 1.819(4) . ?
Mo5 O8 1.952(4) . ?
Mo5 O17 2.401(3) . ?
Mo5 O21 1.806(4) . ?
Mo5 O32 1.683(4) . ?
Mo6 O7 2.090(4) . ?
Mo6 O12 1.680(4) . ?
Mo6 O15 1.762(4) . ?
Mo6 O19 1.854(4) . ?
Mo6 O20 2.103(4) . ?
Mo6 O36 2.249(4) . ?
Mo7 O7 1.808(4) . ?
Mo7 O8 1.968(4) . ?
Mo7 O11 2.170(4) . ?
Mo7 O23 1.807(4) . ?
Mo7 O35 1.693(4) . ?
Mo7 O36 2.399(3) . ?
Mo8 O10 2.087(4) . ?
Mo8 O14 2.287(4) . ?
Mo8 O19 1.973(4) . ?
Mo8 O22 1.749(4) . ?
Mo8 O27 1.950(4) . ?
Mo8 O33 1.687(4) . ?
Mo9 O6 2.112(4) . ?
Mo9 O14 2.301(4) . ?
Mo9 O16 1.747(4) . ?
Mo9 O24 2.013(4) . ?
Mo9 O25 1.692(4) . ?
Mo9 O27 1.907(4) . ?
Mo10 O2 2.186(4) . ?
Mo10 O3 1.987(4) . ?
Mo10 O8 2.160(4) . ?
Mo10 O11 1.981(4) . ?
Mo10 O31 1.699(4) . ?
Mo10 O34 1.733(5) . ?
Ge1 O9 1.759(3) . ?
Ge1 O14 1.750(4) . ?
Ge1 O17 1.753(4) . ?
Ge1 O36 1.753(3) . ?
Co1 O1 2.114(4) 2_635 ?
Co1 O1W 2.066(4) . ?
Co1 O4 2.113(4) 2_635 ?
Co1 O9 2.097(4) . ?
Co1 O16 2.084(4) . ?
Co1 O22 2.075(4) . ?
Co2 O1 2.112(4) 2_635 ?
Co2 O4 2.098(4) . ?
Co2 O9 2.131(4) 2_635 ?
Co2 O9 2.111(4) . ?
Co2 O15 2.063(4) . ?
Co2 O18 2.046(4) 2_635 ?
O1W H1WA 0.8543 . ?
O1W H1WB 0.8222 . ?
Co3 O2W 2.132(5) . ?
Co3 O3W 2.137(5) . ?
Co3 O4W 2.095(5) . ?
Co3 N9 2.136(5) . ?
Co3 N6 2.145(5) 2_756 ?
Co3 N1 2.076(5) . ?
Co4 N10 2.146(5) 2_756 ?
Co4 N10 2.146(5) . ?
Co4 N5 2.116(5) . ?
Co4 N5 2.116(5) 2_756 ?
Co4 N2 2.148(5) 2_756 ?
Co4 N2 2.148(5) . ?
O2W H2WA 0.8403 . ?
O2W H2WB 0.8658 . ?
O3W H3WA 0.8778 . ?
O3W H3WB 0.8786 . ?
O4W H4WA 0.8707 . ?
O4W H4WB 0.8702 . ?
N3 N4 1.412(7) . ?
N3 C1 1.342(7) . ?
N3 C2 1.336(8) . ?
N10 N9 1.380(7) . ?
N10 C6 1.310(8) . ?
N5 N6 1.391(7) . ?
N5 C3 1.299(8) . ?
N2 N1 1.377(7) . ?
N2 C2 1.321(8) . ?
N9 C5 1.302(8) . ?
N7 N8 1.416(7) . ?
N7 C3 1.337(8) . ?
N7 C4 1.337(9) . ?
N6 C4 1.304(8) . ?
N1 C1 1.303(7) . ?
N11 N12 1.409(7) . ?
N11 C5 1.340(9) . ?
N11 C6 1.352(8) . ?
N4 H4A 0.8800 . ?
N4 H4B 0.8800 . ?
N8 H8A 0.8800 . ?
N8 H8B 0.8800 . ?
N12 H12A 0.8800 . ?
N12 H12B 0.8800 . ?
C3 H3 0.9500 . ?
C5 H5 0.9500 . ?
C1 H1 0.9500 . ?
C2 H2 0.9500 . ?
C4 H4 0.9500 . ?
C6 H6 0.9500 . ?
O5W H5WA 0.8198 . ?
O5W H5WB 0.8961 . ?
O6W H6WA 0.8499 . ?
O6W H6WB 0.8427 . ?
O7W H7WA 0.7481 . ?
O7W H7WB 0.8397 . ?
O7WA H7WC 0.8502 . ?
O7WA H7WD 0.8853 . ?
O8W H8WA 0.8502 . ?
O8W H8WB 0.8731 . ?
O9W H9WA 0.8701 . ?
O9W H9WB 0.8701 . ?
O9WA H9WC 0.8697 . ?
O9WA H9WD 0.8700 . ?
O10W H10A 0.8699 . ?
O10W H10B 0.8701 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O5 Mo1 O17 72.01(13) . . ?
O13 Mo1 O5 75.58(15) . . ?
O13 Mo1 O17 72.22(14) . . ?
O18 Mo1 O5 156.28(16) . . ?
O18 Mo1 O13 88.23(16) . . ?
O18 Mo1 O17 86.72(16) . . ?
O18 Mo1 O24 100.39(18) . . ?
O24 Mo1 O5 89.21(16) . . ?
O24 Mo1 O13 157.31(16) . . ?
O24 Mo1 O17 87.24(16) . . ?
O30 Mo1 O5 94.26(18) . . ?
O30 Mo1 O13 94.41(19) . . ?
O30 Mo1 O17 162.61(17) . . ?
O30 Mo1 O18 104.32(19) . . ?
O30 Mo1 O24 103.57(19) . . ?
O6 Mo2 O10 97.94(17) . . ?
O6 Mo2 O14 75.48(14) . . ?
O6 Mo2 O21 87.83(17) . . ?
O6 Mo2 O23 157.01(17) . . ?
O10 Mo2 O14 73.90(15) . . ?
O10 Mo2 O21 154.64(16) . . ?
O10 Mo2 O23 85.16(16) . . ?
O21 Mo2 O14 83.83(14) . . ?
O21 Mo2 O23 80.39(16) . . ?
O23 Mo2 O14 83.64(14) . . ?
O29 Mo2 O6 103.61(18) . . ?
O29 Mo2 O10 101.13(19) . . ?
O29 Mo2 O14 174.65(17) . . ?
O29 Mo2 O21 101.45(18) . . ?
O29 Mo2 O23 98.06(18) . . ?
O1 Mo3 O2 89.05(16) . . ?
O1 Mo3 O3 159.38(17) . . ?
O1 Mo3 O13 99.75(17) . . ?
O1 Mo3 O17 90.78(15) . . ?
O2 Mo3 O3 74.97(15) . . ?
O2 Mo3 O17 79.29(14) . . ?
O3 Mo3 O17 73.72(13) . . ?
O13 Mo3 O2 152.87(17) . . ?
O13 Mo3 O3 89.48(16) . . ?
O13 Mo3 O17 75.01(15) . . ?
O26 Mo3 O1 104.60(19) . . ?
O26 Mo3 O2 101.34(19) . . ?
O26 Mo3 O3 91.48(17) . . ?
O26 Mo3 O13 101.1(2) . . ?
O26 Mo3 O17 164.60(16) . . ?
O2 Mo4 O11 74.52(15) . . ?
O2 Mo4 O36 79.36(15) . . ?
O4 Mo4 O2 88.39(16) . . ?
O4 Mo4 O11 158.26(16) . . ?
O4 Mo4 O20 99.42(17) . . ?
O4 Mo4 O36 89.44(15) . . ?
O11 Mo4 O36 74.49(13) . . ?
O20 Mo4 O2 153.21(16) . . ?
O20 Mo4 O11 90.65(16) . . ?
O20 Mo4 O36 75.16(15) . . ?
O28 Mo4 O2 99.52(19) . . ?
O28 Mo4 O4 103.44(19) . . ?
O28 Mo4 O11 92.74(17) . . ?
O28 Mo4 O20 103.44(19) . . ?
O28 Mo4 O36 167.06(17) . . ?
O3 Mo5 O17 72.71(13) . . ?
O5 Mo5 O3 91.09(17) . . ?
O5 Mo5 O8 150.56(16) . . ?
O5 Mo5 O17 72.84(14) . . ?
O8 Mo5 O3 74.07(16) . . ?
O8 Mo5 O17 78.44(14) . . ?
O21 Mo5 O3 156.75(16) . . ?
O21 Mo5 O5 99.94(18) . . ?
O21 Mo5 O8 86.72(17) . . ?
O21 Mo5 O17 90.96(15) . . ?
O32 Mo5 O3 92.52(18) . . ?
O32 Mo5 O5 104.31(19) . . ?
O32 Mo5 O8 101.67(18) . . ?
O32 Mo5 O17 164.72(18) . . ?
O32 Mo5 O21 104.32(19) . . ?
O7 Mo6 O20 75.37(15) . . ?
O7 Mo6 O36 71.87(14) . . ?
O12 Mo6 O7 93.05(18) . . ?
O12 Mo6 O15 104.17(19) . . ?
O12 Mo6 O19 103.2(2) . . ?
O12 Mo6 O20 95.91(19) . . ?
O12 Mo6 O36 162.14(17) . . ?
O15 Mo6 O7 156.73(17) . . ?
O15 Mo6 O19 100.07(18) . . ?
O15 Mo6 O20 87.22(17) . . ?
O15 Mo6 O36 88.17(16) . . ?
O19 Mo6 O7 90.88(16) . . ?
O19 Mo6 O20 157.03(16) . . ?
O19 Mo6 O36 86.92(15) . . ?
O20 Mo6 O36 71.47(14) . . ?
O7 Mo7 O8 150.36(16) . . ?
O7 Mo7 O11 91.68(17) . . ?
O7 Mo7 O36 73.09(15) . . ?
O8 Mo7 O11 73.15(15) . . ?
O8 Mo7 O36 78.06(14) . . ?
O11 Mo7 O36 72.72(13) . . ?
O23 Mo7 O7 100.80(18) . . ?
O23 Mo7 O8 86.47(17) . . ?
O23 Mo7 O11 156.25(16) . . ?
O23 Mo7 O36 91.53(15) . . ?
O35 Mo7 O7 103.38(19) . . ?
O35 Mo7 O8 102.53(18) . . ?
O35 Mo7 O11 92.24(18) . . ?
O35 Mo7 O23 104.24(19) . . ?
O35 Mo7 O36 164.23(17) . . ?
O10 Mo8 O14 72.68(14) . . ?
O19 Mo8 O10 83.62(15) . . ?
O19 Mo8 O14 85.07(15) . . ?
O22 Mo8 O10 160.91(17) . . ?
O22 Mo8 O14 88.24(16) . . ?
O22 Mo8 O19 94.85(17) . . ?
O22 Mo8 O27 93.00(17) . . ?
O27 Mo8 O10 82.05(15) . . ?
O27 Mo8 O14 73.93(14) . . ?
O27 Mo8 O19 157.32(15) . . ?
O33 Mo8 O10 94.26(18) . . ?
O33 Mo8 O14 165.92(16) . . ?
O33 Mo8 O19 98.96(18) . . ?
O33 Mo8 O22 104.75(19) . . ?
O33 Mo8 O27 99.55(18) . . ?
O6 Mo9 O14 72.92(13) . . ?
O16 Mo9 O6 160.08(16) . . ?
O16 Mo9 O14 87.28(16) . . ?
O16 Mo9 O24 92.54(17) . . ?
O16 Mo9 O27 95.40(17) . . ?
O24 Mo9 O6 83.52(16) . . ?
O24 Mo9 O14 84.33(15) . . ?
O25 Mo9 O6 95.56(18) . . ?
O25 Mo9 O14 167.90(17) . . ?
O25 Mo9 O16 104.34(19) . . ?
O25 Mo9 O24 98.27(19) . . ?
O25 Mo9 O27 100.78(19) . . ?
O27 Mo9 O6 81.62(16) . . ?
O27 Mo9 O14 74.35(14) . . ?
O27 Mo9 O24 156.82(16) . . ?
O3 Mo10 O2 74.74(14) . . ?
O3 Mo10 O8 72.96(16) . . ?
O8 Mo10 O2 85.21(14) . . ?
O11 Mo10 O2 74.38(15) . . ?
O11 Mo10 O3 135.39(16) . . ?
O11 Mo10 O8 73.11(15) . . ?
O31 Mo10 O2 172.81(18) . . ?
O31 Mo10 O3 102.80(18) . . ?
O31 Mo10 O8 87.61(17) . . ?
O31 Mo10 O11 103.82(19) . . ?
O31 Mo10 O34 102.1(2) . . ?
O34 Mo10 O2 85.03(17) . . ?
O34 Mo10 O3 103.0(2) . . ?
O34 Mo10 O8 170.13(17) . . ?
O34 Mo10 O11 105.6(2) . . ?
O14 Ge1 O9 111.45(17) . . ?
O14 Ge1 O17 106.91(17) . . ?
O14 Ge1 O36 106.85(17) . . ?
O17 Ge1 O9 110.16(17) . . ?
O36 Ge1 O9 109.85(16) . . ?
O36 Ge1 O17 111.56(17) . . ?
O1W Co1 O1 95.03(16) . 2_635 ?
O1W Co1 O4 93.24(16) . 2_635 ?
O1W Co1 O9 176.20(17) . . ?
O1W Co1 O16 89.91(16) . . ?
O1W Co1 O22 90.87(17) . . ?
O4 Co1 O1 87.51(15) 2_635 2_635 ?
O9 Co1 O1 83.60(15) . 2_635 ?
O9 Co1 O4 83.17(15) . 2_635 ?
O16 Co1 O1 174.94(16) . 2_635 ?
O16 Co1 O4 91.12(15) . 2_635 ?
O16 Co1 O9 91.40(15) . . ?
O22 Co1 O1 90.61(16) . 2_635 ?
O22 Co1 O4 175.61(16) . 2_635 ?
O22 Co1 O9 92.69(15) . . ?
O22 Co1 O16 90.41(16) . . ?
O1 Co2 O9 91.54(15) 2_635 2_635 ?
O4 Co2 O1 172.16(16) . 2_635 ?
O4 Co2 O9 90.55(14) . . ?
O4 Co2 O9 82.72(15) . 2_635 ?
O9 Co2 O1 83.32(15) . 2_635 ?
O9 Co2 O9 81.63(15) . 2_635 ?
O15 Co2 O1 93.17(16) . 2_635 ?
O15 Co2 O4 92.20(16) . . ?
O15 Co2 O9 173.71(15) . 2_635 ?
O15 Co2 O9 94.77(15) . . ?
O18 Co2 O1 91.70(15) 2_635 2_635 ?
O18 Co2 O4 93.82(15) 2_635 . ?
O18 Co2 O9 92.07(15) 2_635 2_635 ?
O18 Co2 O9 171.83(16) 2_635 . ?
O18 Co2 O15 91.96(16) 2_635 . ?
Mo3 O1 Co1 129.0(2) . 2_635 ?
Mo3 O1 Co2 130.9(2) . 2_635 ?
Co2 O1 Co1 96.06(15) 2_635 2_635 ?
Co1 O1W H1WA 109.4 . . ?
Co1 O1W H1WB 127.5 . . ?
H1WA O1W H1WB 116.7 . . ?
Mo3 O2 Mo4 152.5(2) . . ?
Mo3 O2 Mo10 103.53(16) . . ?
Mo4 O2 Mo10 103.78(17) . . ?
Mo5 O3 Mo3 111.95(16) . . ?
Mo10 O3 Mo3 103.18(16) . . ?
Mo10 O3 Mo5 104.42(18) . . ?
Mo4 O4 Co1 128.5(2) . 2_635 ?
Mo4 O4 Co2 131.8(2) . . ?
Co2 O4 Co1 97.01(15) . 2_635 ?
Mo5 O5 Mo1 119.19(18) . . ?
Mo2 O6 Mo9 119.48(19) . . ?
Mo7 O7 Mo6 119.80(19) . . ?
Mo5 O8 Mo7 149.5(2) . . ?
Mo5 O8 Mo10 104.93(18) . . ?
Mo7 O8 Mo10 105.53(17) . . ?
Ge1 O9 Co1 119.72(19) . . ?
Ge1 O9 Co2 120.23(19) . . ?
Ge1 O9 Co2 120.11(18) . 2_635 ?
Co1 O9 Co2 96.48(15) . 2_635 ?
Co1 O9 Co2 96.58(14) . . ?
Co2 O9 Co2 98.37(15) . 2_635 ?
Mo2 O10 Mo8 120.1(2) . . ?
Mo7 O11 Mo4 110.70(16) . . ?
Mo10 O11 Mo4 104.17(17) . . ?
Mo10 O11 Mo7 104.70(17) . . ?
Mo3 O13 Mo1 115.7(2) . . ?
Mo8 O14 Mo2 92.52(13) . . ?
Mo8 O14 Mo9 91.77(13) . . ?
Mo9 O14 Mo2 91.65(12) . . ?
Ge1 O14 Mo2 128.41(18) . . ?
Ge1 O14 Mo8 121.44(18) . . ?
Ge1 O14 Mo9 121.51(19) . . ?
Mo6 O15 Co2 139.9(2) . . ?
Mo9 O16 Co1 137.9(2) . . ?
Mo1 O17 Mo3 94.16(14) . . ?
Mo1 O17 Mo5 94.07(12) . . ?
Mo3 O17 Mo5 99.03(13) . . ?
Ge1 O17 Mo1 122.31(18) . . ?
Ge1 O17 Mo3 120.51(17) . . ?
Ge1 O17 Mo5 120.42(18) . . ?
Mo1 O18 Co2 142.9(2) . 2_635 ?
Mo6 O19 Mo8 146.4(2) . . ?
Mo4 O20 Mo6 116.53(18) . . ?
Mo5 O21 Mo2 154.9(2) . . ?
Mo8 O22 Co1 138.5(2) . . ?
Mo7 O23 Mo2 153.5(2) . . ?
Mo1 O24 Mo9 144.8(2) . . ?
Mo9 O27 Mo8 117.28(19) . . ?
Mo4 O36 Mo7 98.98(13) . . ?
Mo6 O36 Mo4 94.28(13) . . ?
Mo6 O36 Mo7 93.10(13) . . ?
Ge1 O36 Mo4 120.69(18) . . ?
Ge1 O36 Mo6 122.36(18) . . ?
Ge1 O36 Mo7 120.84(17) . . ?
O2W Co3 O3W 88.9(2) . . ?
O2W Co3 N9 89.1(2) . . ?
O2W Co3 N6 177.0(2) . 2_756 ?
O3W Co3 N6 92.5(2) . 2_756 ?
O4W Co3 O2W 86.7(2) . . ?
O4W Co3 O3W 82.6(2) . . ?
O4W Co3 N9 98.2(2) . . ?
O4W Co3 N6 90.8(2) . 2_756 ?
N9 Co3 O3W 177.8(2) . . ?
N9 Co3 N6 89.6(2) . 2_756 ?
N1 Co3 O2W 88.5(2) . . ?
N1 Co3 O3W 88.97(19) . . ?
N1 Co3 O4W 170.4(2) . . ?
N1 Co3 N9 90.05(19) . . ?
N1 Co3 N6 94.23(19) . 2_756 ?
N10 Co4 N10 180.0 2_756 . ?
N10 Co4 N2 89.93(18) . 2_756 ?
N10 Co4 N2 90.07(18) 2_756 2_756 ?
N10 Co4 N2 89.93(18) 2_756 . ?
N10 Co4 N2 90.07(18) . . ?
N5 Co4 N10 89.18(18) . 2_756 ?
N5 Co4 N10 90.82(18) . . ?
N5 Co4 N10 89.18(18) 2_756 . ?
N5 Co4 N10 90.82(18) 2_756 2_756 ?
N5 Co4 N5 180.0 2_756 . ?
N5 Co4 N2 90.87(19) 2_756 . ?
N5 Co4 N2 90.87(19) . 2_756 ?
N5 Co4 N2 89.13(19) . . ?
N5 Co4 N2 89.13(19) 2_756 2_756 ?
N2 Co4 N2 180.0 2_756 . ?
Co3 O2W H2WA 110.8 . . ?
Co3 O2W H2WB 110.2 . . ?
H2WA O2W H2WB 130.6 . . ?
Co3 O3W H3WA 110.7 . . ?
Co3 O3W H3WB 111.2 . . ?
H3WA O3W H3WB 102.8 . . ?
Co3 O4W H4WA 111.1 . . ?
Co3 O4W H4WB 109.7 . . ?
H4WA O4W H4WB 102.9 . . ?
C1 N3 N4 127.3(5) . . ?
C2 N3 N4 125.5(5) . . ?
C2 N3 C1 107.2(5) . . ?
N9 N10 Co4 126.3(4) . . ?
C6 N10 Co4 125.8(4) . . ?
C6 N10 N9 107.9(5) . . ?
N6 N5 Co4 127.1(4) . . ?
C3 N5 Co4 124.0(4) . . ?
C3 N5 N6 107.1(5) . . ?
N1 N2 Co4 122.7(3) . . ?
C2 N2 Co4 129.2(4) . . ?
C2 N2 N1 107.8(5) . . ?
N10 N9 Co3 122.7(4) . . ?
C5 N9 Co3 130.7(4) . . ?
C5 N9 N10 106.5(5) . . ?
C3 N7 N8 126.7(6) . . ?
C4 N7 N8 127.0(6) . . ?
C4 N7 C3 106.3(5) . . ?
N5 N6 Co3 121.8(4) . 2_756 ?
C4 N6 Co3 131.2(5) . 2_756 ?
C4 N6 N5 106.4(5) . . ?
N2 N1 Co3 127.5(3) . . ?
C1 N1 Co3 125.9(4) . . ?
C1 N1 N2 106.6(5) . . ?
C5 N11 N12 125.3(6) . . ?
C5 N11 C6 106.1(5) . . ?
C6 N11 N12 128.6(6) . . ?
N3 N4 H4A 120.0 . . ?
N3 N4 H4B 120.0 . . ?
H4A N4 H4B 120.0 . . ?
N7 N8 H8A 120.0 . . ?
N7 N8 H8B 120.0 . . ?
H8A N8 H8B 120.0 . . ?
N11 N12 H12A 120.0 . . ?
N11 N12 H12B 120.0 . . ?
H12A N12 H12B 120.0 . . ?
N5 C3 N7 110.0(6) . . ?
N5 C3 H3 125.0 . . ?
N7 C3 H3 125.0 . . ?
N9 C5 N11 110.6(6) . . ?
N9 C5 H5 124.7 . . ?
N11 C5 H5 124.7 . . ?
N3 C1 H1 125.1 . . ?
N1 C1 N3 109.9(5) . . ?
N1 C1 H1 125.1 . . ?
N3 C2 H2 125.8 . . ?
N2 C2 N3 108.4(5) . . ?
N2 C2 H2 125.8 . . ?
N7 C4 H4 124.9 . . ?
N6 C4 N7 110.2(6) . . ?
N6 C4 H4 124.9 . . ?
N10 C6 N11 108.9(6) . . ?
N10 C6 H6 125.5 . . ?
N11 C6 H6 125.5 . . ?
H5WA O5W H5WB 86.7 . . ?
H6WA O6W H6WB 96.7 . . ?
H7WA O7W H7WB 111.7 . . ?
H7WC O7WA H7WD 109.6 . . ?
H8WA O8W H8WB 107.8 . . ?
H9WA O9W H9WB 104.5 . . ?
H9WC O9WA H9WD 104.5 . . ?
H10A O10W H10B 104.5 . . ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
_geom_hbond_publ_flag
O1W H1WA O5W 0.85 1.79 2.595(7) 156.6 2_646 yes
O2W H2WB O7W 0.87 1.90 2.680(12) 149.8 . yes
O2W H2WB O7WA 0.87 1.86 2.703(16) 164.5 . yes
O5W H5WA O10 0.82 2.07 2.741(7) 139.3 1_565 yes
O6W H6WA O9W 0.85 1.99 2.82(3) 163.7 2_656 yes
O6W H6WA O9WA 0.85 1.85 2.70(5) 170.4 2_656 yes
O7W H7WA O3W 0.75 2.12 2.855(15) 167.7 2_757 yes
O7W H7WB O30 0.84 2.06 2.808(11) 148.5 1_666 yes
O7WA H7WC O20 0.85 2.04 2.822(13) 152.6 1_566 yes
O7WA H7WD O30 0.89 1.97 2.833(13) 164.2 1_666 yes
O9WA H9WD O8W 0.87 2.00 2.85(4) 165.4 1_565 yes

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O1 Mo3 O13 Mo1 73.8(2) . . . . ?
O2 Mo3 O1 Co1 -42.2(3) . . . 2_635 ?
O2 Mo3 O1 Co2 109.8(3) . . . 2_635 ?
O2 Mo3 O13 Mo1 -33.5(4) . . . . ?
O2 Mo4 O4 Co1 45.1(2) . . . 2_635 ?
O2 Mo4 O4 Co2 -111.9(3) . . . . ?
O2 Mo4 O20 Mo6 32.2(5) . . . . ?
O3 Mo3 O1 Co1 -80.9(5) . . . 2_635 ?
O3 Mo3 O1 Co2 71.1(6) . . . 2_635 ?
O3 Mo3 O13 Mo1 -87.7(2) . . . . ?
O3 Mo5 O5 Mo1 83.3(2) . . . . ?
O3 Mo5 O21 Mo2 4.6(9) . . . . ?
O4 Mo4 O20 Mo6 -73.2(2) . . . . ?
O5 Mo1 O18 Co2 7.4(7) . . . 2_635 ?
O5 Mo1 O24 Mo9 -138.3(4) . . . . ?
O5 Mo5 O21 Mo2 121.8(5) . . . . ?
O6 Mo2 O10 Mo8 64.5(2) . . . . ?
O6 Mo9 O16 Co1 37.1(7) . . . . ?
O7 Mo6 O15 Co2 -16.5(7) . . . . ?
O7 Mo6 O19 Mo8 136.5(4) . . . . ?
O7 Mo7 O23 Mo2 -120.9(5) . . . . ?
O8 Mo5 O5 Mo1 25.0(5) . . . . ?
O8 Mo5 O21 Mo2 -29.3(5) . . . . ?
O8 Mo7 O7 Mo6 -26.5(5) . . . . ?
O8 Mo7 O23 Mo2 30.1(5) . . . . ?
O9 Ge1 O14 Mo2 -179.4(2) . . . . ?
O9 Ge1 O14 Mo8 57.2(2) . . . . ?
O9 Ge1 O14 Mo9 -57.5(2) . . . . ?
O9 Ge1 O17 Mo1 59.4(2) . . . . ?
O9 Ge1 O17 Mo3 -58.8(2) . . . . ?
O9 Ge1 O17 Mo5 177.33(18) . . . . ?
O9 Ge1 O36 Mo4 58.9(2) . . . . ?
O9 Ge1 O36 Mo6 -59.8(2) . . . . ?
O9 Ge1 O36 Mo7 -176.69(18) . . . . ?
O10 Mo2 O6 Mo9 -64.9(2) . . . . ?
O10 Mo8 O22 Co1 -25.3(7) . . . . ?
O11 Mo4 O4 Co1 82.8(5) . . . 2_635 ?
O11 Mo4 O4 Co2 -74.2(5) . . . . ?
O11 Mo4 O20 Mo6 87.5(2) . . . . ?
O11 Mo7 O7 Mo6 -84.2(2) . . . . ?
O11 Mo7 O23 Mo2 -0.5(8) . . . . ?
O12 Mo6 O15 Co2 -153.0(3) . . . . ?
O12 Mo6 O19 Mo8 -130.1(4) . . . . ?
O13 Mo1 O18 Co2 53.8(4) . . . 2_635 ?
O13 Mo1 O24 Mo9 -91.0(5) . . . . ?
O13 Mo3 O1 Co1 163.6(3) . . . 2_635 ?
O13 Mo3 O1 Co2 -44.4(3) . . . 2_635 ?
O14 Mo2 O6 Mo9 6.09(19) . . . . ?
O14 Mo2 O10 Mo8 -7.85(18) . . . . ?
O14 Mo8 O22 Co1 -24.9(3) . . . . ?
O14 Mo9 O16 Co1 30.8(3) . . . . ?
O14 Ge1 O9 Co1 0.5(3) . . . . ?
O14 Ge1 O9 Co2 119.3(2) . . . 2_635 ?
O14 Ge1 O9 Co2 -118.5(2) . . . . ?
O14 Ge1 O17 Mo1 -61.9(2) . . . . ?
O14 Ge1 O17 Mo3 179.96(18) . . . . ?
O14 Ge1 O17 Mo5 56.1(2) . . . . ?
O14 Ge1 O36 Mo4 179.88(18) . . . . ?
O14 Ge1 O36 Mo6 61.3(2) . . . . ?
O14 Ge1 O36 Mo7 -55.7(2) . . . . ?
O15 Mo6 O19 Mo8 -22.8(4) . . . . ?
O17 Mo1 O18 Co2 -18.5(4) . . . 2_635 ?
O17 Mo1 O24 Mo9 -66.3(4) . . . . ?
O17 Mo3 O1 Co1 -121.4(3) . . . 2_635 ?
O17 Mo3 O1 Co2 30.5(3) . . . 2_635 ?
O17 Mo3 O13 Mo1 -14.37(17) . . . . ?
O17 Mo5 O5 Mo1 11.82(18) . . . . ?
O17 Mo5 O21 Mo2 49.0(5) . . . . ?
O17 Ge1 O9 Co1 -118.0(2) . . . . ?
O17 Ge1 O9 Co2 123.0(2) . . . . ?
O17 Ge1 O9 Co2 0.8(3) . . . 2_635 ?
O17 Ge1 O14 Mo2 -59.0(3) . . . . ?
O17 Ge1 O14 Mo8 177.59(18) . . . . ?
O17 Ge1 O14 Mo9 62.9(2) . . . . ?
O17 Ge1 O36 Mo4 -63.6(2) . . . . ?
O17 Ge1 O36 Mo6 177.79(18) . . . . ?
O17 Ge1 O36 Mo7 60.9(2) . . . . ?
O18 Mo1 O24 Mo9 19.9(4) . . . . ?
O19 Mo6 O15 Co2 100.4(3) . . . . ?
O19 Mo8 O22 Co1 -109.8(3) . . . . ?
O20 Mo4 O4 Co1 -160.7(2) . . . 2_635 ?
O20 Mo4 O4 Co2 42.4(3) . . . . ?
O20 Mo6 O15 Co2 -57.6(3) . . . . ?
O20 Mo6 O19 Mo8 84.2(5) . . . . ?
O21 Mo2 O6 Mo9 90.3(2) . . . . ?
O21 Mo2 O10 Mo8 -37.3(5) . . . . ?
O21 Mo5 O5 Mo1 -76.1(2) . . . . ?
O23 Mo2 O6 Mo9 31.4(5) . . . . ?
O23 Mo2 O10 Mo8 -92.6(2) . . . . ?
O23 Mo7 O7 Mo6 75.5(2) . . . . ?
O24 Mo1 O18 Co2 -105.1(4) . . . 2_635 ?
O24 Mo9 O16 Co1 115.0(3) . . . . ?
O25 Mo9 O16 Co1 -145.8(3) . . . . ?
O26 Mo3 O1 Co1 59.3(3) . . . 2_635 ?
O26 Mo3 O1 Co2 -148.7(3) . . . 2_635 ?
O26 Mo3 O13 Mo1 -179.1(2) . . . . ?
O27 Mo8 O22 Co1 48.9(3) . . . . ?
O27 Mo9 O16 Co1 -43.2(3) . . . . ?
O28 Mo4 O4 Co1 -54.3(3) . . . 2_635 ?
O28 Mo4 O4 Co2 148.7(3) . . . . ?
O28 Mo4 O20 Mo6 -179.5(2) . . . . ?
O29 Mo2 O6 Mo9 -168.5(2) . . . . ?
O29 Mo2 O10 Mo8 170.1(2) . . . . ?
O30 Mo1 O18 Co2 147.8(4) . . . 2_635 ?
O30 Mo1 O24 Mo9 127.5(4) . . . . ?
O32 Mo5 O5 Mo1 176.2(2) . . . . ?
O32 Mo5 O21 Mo2 -130.6(5) . . . . ?
O33 Mo8 O22 Co1 149.6(3) . . . . ?
O35 Mo7 O7 Mo6 -176.9(2) . . . . ?
O35 Mo7 O23 Mo2 132.1(5) . . . . ?
O36 Mo4 O4 Co1 124.5(2) . . . 2_635 ?
O36 Mo4 O4 Co2 -32.5(3) . . . . ?
O36 Mo4 O20 Mo6 13.73(17) . . . . ?
O36 Mo6 O15 Co2 13.9(3) . . . . ?
O36 Mo6 O19 Mo8 64.7(4) . . . . ?
O36 Mo7 O7 Mo6 -12.79(19) . . . . ?
O36 Mo7 O23 Mo2 -47.9(5) . . . . ?
O36 Ge1 O9 Co1 118.8(2) . . . . ?
O36 Ge1 O9 Co2 -122.5(2) . . . 2_635 ?
O36 Ge1 O9 Co2 -0.3(3) . . . . ?
O36 Ge1 O14 Mo2 60.5(3) . . . . ?
O36 Ge1 O14 Mo8 -62.9(2) . . . . ?
O36 Ge1 O14 Mo9 -177.52(18) . . . . ?
O36 Ge1 O17 Mo1 -178.35(18) . . . . ?
O36 Ge1 O17 Mo3 63.5(2) . . . . ?
O36 Ge1 O17 Mo5 -60.4(2) . . . . ?
Co3 N9 C5 N11 176.9(4) . . . . ?
Co3 N6 C4 N7 171.0(4) 2_756 . . . ?
Co3 N1 C1 N3 178.3(4) . . . . ?
Co4 N10 N9 Co3 0.7(6) . . . . ?
Co4 N10 N9 C5 178.8(4) . . . . ?
Co4 N10 C6 N11 -178.6(4) . . . . ?
Co4 N5 N6 Co3 -7.3(6) . . . 2_756 ?
Co4 N5 N6 C4 164.1(4) . . . . ?
Co4 N5 C3 N7 -164.8(4) . . . . ?
Co4 N2 N1 Co3 -4.6(6) . . . . ?
Co4 N2 N1 C1 174.8(4) . . . . ?
Co4 N2 C2 N3 -173.1(4) . . . . ?
N10 N9 C5 N11 -1.0(7) . . . . ?
N5 N6 C4 N7 0.8(7) . . . . ?
N2 N1 C1 N3 -1.2(6) . . . . ?
N9 N10 C6 N11 -1.0(7) . . . . ?
N6 N5 C3 N7 1.0(7) . . . . ?
N1 N2 C2 N3 1.5(6) . . . . ?
N4 N3 C1 N1 -178.8(5) . . . . ?
N4 N3 C2 N2 178.7(5) . . . . ?
N8 N7 C3 N5 177.7(5) . . . . ?
N8 N7 C4 N6 -178.4(6) . . . . ?
N12 N11 C5 N9 -178.4(6) . . . . ?
N12 N11 C6 N10 179.1(6) . . . . ?
C3 N5 N6 Co3 -172.4(4) . . . 2_756 ?
C3 N5 N6 C4 -1.1(7) . . . . ?
C3 N7 C4 N6 -0.2(7) . . . . ?
C5 N11 C6 N10 0.4(7) . . . . ?
C1 N3 C2 N2 -2.2(7) . . . . ?
C2 N3 C1 N1 2.1(7) . . . . ?
C2 N2 N1 Co3 -179.6(4) . . . . ?
C2 N2 N1 C1 -0.2(6) . . . . ?
C4 N7 C3 N5 -0.5(7) . . . . ?
C6 N10 N9 Co3 -176.9(4) . . . . ?
C6 N10 N9 C5 1.2(6) . . . . ?
C6 N11 C5 N9 0.4(7) . . . . ?

_olex2_submission_special_instructions 'No special instructions were received'
